* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project
PHYSICAL REVIEW B VOLUME 62, NUMBER 6 1 AUGUST 2000-II Nonlinear transport current flow in superconductors with planar obstacles Alex Gurevich and Mark Friesen Applied Superconductivity Center, University of Wisconsin, Madison, Wisconsin 53706 共Received 13 January 2000兲 We present a detailed description of a hodograph method, which enables us to calculate analytically the two-dimensional distributions of the electric field E(r) and transport current density J(r) in superconductors, taking into account their highly nonlinear E-J characteristics. The method gives a unique solution E(r) of nonlinear steady-state Maxwell’s equations for given boundary conditions, showing applicability limits of the critical state model and pointing out where it breaks down. The nonlinear problem of calculation of J(r) by the hodograph method reduces to solving a linear equation for the electric potential (E), or the current stream function (E) as a function of E. For the power-law characteristics E⫽E c (J/J c ) n , calculation of E(r) and J(r) can be mapped onto solutions of the London equation with the inverse screening length ␤ ⫽(n ⫺1)/2冑n in the hodograph space (E x E y ). We give general methods of solving the hodograph equations and obtain closed-form analytical solutions for particular current flows. The method is applied to calculate distributions of E(r) and dissipation in superconductors with macroscopic planar defects, such as high-angle grain boundaries, microcracks, etc. Current patterns around planar obstacles are shown to break up into domains of different orientations of J, separated by current domain walls. We calculate the structure of the current domain walls, whose width depends both on the geometry of current flow and the exponent n. These domain walls differ from the current discontinuity lines of the Bean model even in the limit n→⬁. We obtained a solution for current flow past a planar defect of length 2a in an infinite superconductor and showed that the defect causes strong local electric-field enhancement and long-range disturbances of E(r) on length scales L⬜ ⬃an Ⰷa and L 储 ⬃a 冑nⰇa perpendicular and parallel to the mean current flow, respectively. This solution also exhibits large stagnation regions of magnetic flux near planar defects, universal distributions of J(r) in the critical state limit, n→⬁, and local flux flow regions near the edges. We calculate Joule heating for nonlinear current flow and show that planar defects cause significant excess dissipation, which affects ac losses and local thermal instabilities in superconductors. I. INTRODUCTION Macroscopic electrodynamics of type-II superconductors in the mixed state is determined by the pinning and thermally activated creep of vortex structures, which gives rise to a weakly dissipative critical current, irreversible magnetization, and slow current relaxation 共flux creep兲. These phenomena manifest themselves on length scales much larger than the Larkin pinning correlation length L c , on which the critical state is formed.1 On these macroscopic scales LⰇL c , the only material characteristic which determines the behavior of superconductors in electromagnetic fields is the nonlinear local relation between the electric field E and current density J, J⫽ E J共 E 兲. E enable one to calculate the evolution of nonuniform distributions of E(r,t) and B(r,t) and thus to describe macroscopic magnetic, transport, and relaxation phenomena in superconductors.1–4 A type-II superconductor in the mixed state exhibits a highly nonlinear E(J) dependence below a critical current density J c , which separates regimes of flux flow at J⬎J c and flux creep at J⬍J c 共Fig. 1兲. The crucial behavior of E(J) at J⬍J c is determined by thermally activated vortex creep: 冋 E 共 J 兲 ⫽E c exp ⫺ 册 U 共 J,T,B 兲 , T 共3兲 共1兲 Here E(r,t) and J(r,t) refer to the macroscopic electric field and current density averaged over all relevant intrinsic scales of pinned vortex structure, such as intervortex spacing, pinning correlation lengths, etc. We consider an isotropic E-J relation 共1兲, which, for example, models the nearly twodimensional 共2D兲 current flow in the ab plane of layered high-temperature superconductors 共HTS’s兲. Equation 共1兲, combined with the Maxwell equations t B⫽⫺ⵜ⫻E, ⵜ⫻H⫽J共 E兲 , 0163-1829/2000/62共6兲/4004共22兲/$15.00 共2兲 PRB 62 FIG. 1. E-J characteristic of a type-II superconductor. 4004 ©2000 The American Physical Society PRB 62 NONLINEAR TRANSPORT CURRENT FLOW IN . . . 4005 FIG. 2. Percolative current flow in polycrystals. Currentblocking high-angle grain boundaries are shown as solid lines, while low-angle grain boundaries, transparent to current flow, are shown as dashed lines. where U(J,T,B) is an activation barrier, which depends on J, the temperature T, and the magnetic induction, B. Here E c is a conditional electric-field criterion, which defines an apparent J c by the relation, U(J c ,T,B)⫽0. For instance, vortex glass/collective creep models1 give a divergent dependence U⫽U c 关 (J c /J) ⫺1 兴 at small JⰆJ c , which has been observed in transport and magnetization measurements on HTS’s.3 Similar though less singular logarithmic dependence U⫽U c ln(Jc /J) corresponds to power-law E-J characteristics, E⫽E c (J/J c ) n with n(T,B)⫽U c /T⬃3 –30. It is a good approximation of the observed E(J) for type-II superconductors, especially for layered Bi-based HTS’s.5 If the distribution of J(r) varies on spatial scales greater than L c , a superconductor can be regarded as a highly nonlinear, nonuniform conductor with a local characteristic E(J,r). For example, Eqs. 共1兲 and 共2兲 describe nonlinear transport in superconductors with macroscopic obstacles or percolative current flow in HTS polycrystals with grain sizes ⰇL c 共Fig. 2兲. This case is important for understanding current-limiting mechanisms of HTS’s, which, in addition to grain boundaries, often contain other macroscopic defects, such as second phase precipitates, microcracks, and regions of local nonstoichiometry on scales of order 10–1000 m.6 These current-blocking obstacles cause macroscopically nonuniform distributions of transport and magnetization currents, as revealed by magneto-optical imaging of HTS’s.7–10 In turn, even comparatively weak inhomogeneities of local J(r) can cause exponentially strong variations of the electric field, E(r)⬀J exp关⫺U(J)/T兴, which radically change global characteristics of superconductors J̄(Ē,B,T) observed in experiment. Thus the behavior of J̄(Ē,B,T) can be different from local characteristics 共1兲 determined by thermally activated vortex dynamics and pinning on mesoscopic scales, L⬍L c . For instance, the relation between global J̄(Ē,B,T) characteristics and local J(E,r) is rather complex, even in nonuniform Ohmic conductors.11 This is even more so for superconductors, where the global and local characteristics can exhibit different dependencies on E, B, and T, because the nonlinearity of E(J) makes the effective current-carrying cross section dependent on T, B, and E.12–15 Shown in Fig. 3 are examples of 2D current flows for different cases, which could be regarded as elementary ‘‘building blocks’’ of a more general percolative network in Fig. 2. The geometries shown in Fig. 3 are also quite common in experimental studies of resistive states in supercon- FIG. 3. Characteristic cases of the 2D nonlinear current flow solvable by the hodograph method. ductors, thin-film superconducting electronic circuits and HTS conductors for power applications. For instance, Fig. 3共a兲 shows a superconducting film with a strong currentlimiting planar defect 共microcrack or high angle grain boundary兲. The case in Fig. 3共a兲 is also mathematically analogous to that in Fig. 3共b兲, which shows current flow through a faceted grain boundary with alternating segments of different J c values. Other common geometries include the current injector 共or magnetic flux transformer兲 关Fig. 3共c兲兴 and the microbridge 关Fig. 3共d兲兴. In all cases shown in Figs. 2 and 3, the electric field and current density are inhomogeneous on macroscopic scales and have singularities near the sharp edges and corners. Calculations of the global E-J characteristics then require solving Eqs. 共1兲 and 共2兲. The highly nonlinear Eqs. 共1兲 and 共2兲 represent a difficult mathematical problem, which has, to our knowledge, not so far been addressed analytically, except for a few results on 1D flux penetration16 and flux creep dynamics.4 Extensive numerical studies of the dynamics of flux penetration by Brandt17 have revealed many important features of nonlinear flux dynamics in superconductors, such as narrow domain walls separating regions with different directions of current flow, nonlocal flux diffusion in thin samples, the influence of geometrical barrier, etc. On the other hand, the problem of 2D steady-state transport current flow has remained unsolved, because even numerical simulations of Eqs. 共1兲 and 共2兲 become exceedingly time consuming as the nonlinearity of E(J) increases. For large n values, even weak spatial variations of J(r) around planar defects in Fig. 2 produce exponentially large variations of electric field E(r) ⫽E c 关 J(r)/J c 兴 n . This fact along with singularities of J(r) and E(r) at the edges considerably complicate numerical analysis of Eqs. 共1兲 and 共2兲, making it necessary to develop an analytical method for solving Eqs. 共1兲 and 共2兲. An approximate method for obtaining current distribution in superconductors is given by the Bean critical state model,18,19 which replaces the real E(J) curve 共1兲 by a stepwise dependence: J⫽EJ c /E for E⬎0, and E⫽0 for J⬍J c 共Fig. 1兲. This model may be regarded as an extreme limit of the power-law characteristic, E⫽E c (J/J c ) n for n→⬁,17 which enables analytical solutions for J(r) for some simple cases 共Fig. 4兲. These solutions exhibit characteristic ‘‘discon- 4006 ALEX GUREVICH AND MARK FRIESEN PRB 62 the infinite extent of current perturbations around local inhomogeneities 共Fig. 4兲, the zero thickness of the d lines, and multiple solutions of the Bean model, fixing a unique steadystate transport current distribution for given boundary conditions. However, the account of the nonlinear E(J) requires solving the following nonlinear equation for the scalar potential : 冋 div FIG. 4. Magnetization current flows predicted by the Bean model. Top: long slab in a parallel magnetic field. Bottom: current flow around a cylindrical void 共Ref. 19兲. Dashed lines show the parabolic d lines, on which J sharply changes direction. Current streamlines between the d lines are circular, and centered in the void. tinuity’’ lines (d lines兲, along which the current abruptly changes direction. Another feature of this model is that finite-size defects can cause current disturbances of infinite range, as it occurs for current flow past a cylindrical void, in which case parabolic d lines extend to infinity19,20 关Fig. 4共b兲兴. Both the zero thickness of the d lines and the infinite spatial scale of current perturbations are consequences of the zero resistivity for the idealized Bean’s E-J characteristic in the whole interval 0⬍J⭐J c . In this case, solving steady-state Eqs. 共2兲 becomes an ill-defined mathematical problem, which reduces to the only condition of current continuity, div J⫽0, provided that J⭐J c . These conditions can be satisfied by many different current distributions for a given sample geometry, since the selection of Bean’s solutions for J(r) is due to initial conditions. For example, the initial distribution of electric field E(r) can be induced by increasing external magnetic field. Once the initial conditions are fixed by the magnetic prehistory, the distribution of J(r) stays frozen indefinitely. The inherent hysteresis of the critical state makes the Bean model inappropriate for calculations of steady-state transport current flow around planar obstacles in Figs. 2 and 3, for which the current-carrying cross section varies along a superconductor. In this case current path inevitably breaks into regions in the critical state, J⫽J c , and subcritical regions, with 0⬍J⬍J c . However, the particular distribution of these regions depends on initial conditions and thus cannot be calculated by solving the steady-state equations, div J⫽0 and J⭐J c . This unphysical situation results from the fact that the Bean model ignores the necessary condition ⵜ⫻E⫽0, which can only be satisfied by taking account of the highly nonlinear E-J characteristics 共1兲. Although exponentially small at J⬍J c , the nonzero electric field plays an important role, since solving Eqs. 共1兲 now becomes a welldefined mathematical problem, for which each nonzero value of J corresponds to a certain E. The account of E eliminates 册 ⵜ J 共 兩 ⵜ 兩 兲 ⫽0, 兩ⵜ兩 共4兲 which is obtained by substituting E⫽⫺ⵜ into Eq. 共1兲 and then into div J⫽0. The 2D Eq. 共4兲 is rather difficult to solve either analytically or numerically. Recently we proposed an analytical method to calculate 2D steady-state transport current flow in superconductors with the account of their nonlinear E(J) characteristics.21,22 The method is based on a hodograph transformation, developed at the beginning of the 20th century to describe compressible gas flow.23,24 In Ref. 21 the hodograph method was developed as to describe current flow in anisotropic superconductors. Using this method, analytical steady-state solutions of Eqs. 共1兲 and 共2兲 for current flow past a planar defect were obtained for the power-law E-J characteristics.22 The essence of the hodograph method is the following. Instead of dealing with the highly nonlinear equation for (r) in the coordinate space, we change variables and express (r) as a function of the electric field E: 共 r兲 → 共 E兲 . 共5兲 The hodograph transformation 共5兲 reduces the nonlinear Eq. 共4兲 for (r) to a linear equation for (E). In turn, the equation for (E) can be further reduced to other well-studied linear partial differential equations, such as Thomas-Fermi or London equations, whose known solutions can be used to obtain exact solutions for 2D current flows in nonlinear conductors. For example, the nonlinear current flow around a planar defect can be mapped onto a solution of the London equation, which describes the magnetic-field distribution from a fictitious fluxon in a film with cuts. Here the nonlinearity of the power-law characteristic E⫽E c (J/J c ) n manifests itself in the nonzero effective ‘‘screening length’’ l ⫽2 冑n/(n⫺1). These analogies enables one to use known solutions of the London, Debye, or diffusion equations 共see below兲 to obtain analytical solutions for the 2D nonlinear current flows in superconductors with macroscopic defects.22 The hodograph method enables us to resolve the ambiguities of the Bean model and address analytically features of 2D nonlinear transport current flow. In particular, it gives a unique steady-state distribution J(r) for a given sample geometry and shows that current flow breaks into domains with different orientations of J separated by current domain walls reminiscent of the d lines of the Bean model. However, there are important differences between the current domain walls and the d lines. First of all, the domain walls have an internal structure and a varying width, which depends both on the n value and the geometry of current flow. For instance, for current flow past a void in Fig. 4, the width of the domain PRB 62 NONLINEAR TRANSPORT CURRENT FLOW IN . . . walls increases with the distance from the void. It is the broadening of the domain walls, which provides the decay of current perturbations caused by the defect size a on a finite length L⬜ ⬃an, much larger than a, if nⰇ1. Moreover, the current domain walls described by exact hodograph solutions remain different from the phenomenological d lines even in the critical state limit, n→⬁. In this case current flow near domain walls exhibits no discontinuities in the tangential components of J(x,y) thus satisfying ⵜ⫻E⫽0. In this and a subsequent paper25 we present a detailed description of the hodograph method and calculate various steady-state 2D transport current flow in superconductors. In this paper we focus on general features of current flow in isotropic nonlinear conductors illustrated by characteristic examples, which show how the method works. We present exact solutions of Eq. 共4兲, which reveal new length scales of nonlinear current flow and the structure of current domain walls. The second part of this work25 is devoted to calculations of the distributions of J(r) and E(r) for restricted geometries shown in Fig. 3. Because of the long-range disturbances of the E(x,y) near defects in superconductors,22 the effect of the sample geometry becomes crucial and in many cases completely dominates the global nonlinear current transport. These results enable us to calculate global E-J characteristics and dissipation due to defects, which also pertain to the problems of current-carrying capability, ac losses, and thermal stability of superconductors. In addition to superconductors, the hodograph method can also be applied to calculations of nonuniform current flow in other nonlinear media, such as semiconductors, plasma, etc. For instance, E-J characteristics of gas or semiconductor plasma at high electric fields can be approximated by the power-law dependence, E⬀J n , with nⰆ1.26 The paper is organized as follows. In Sec. II we consider features of nonlinear current flow and discuss conditions, under which the steady-state current distributions in superconductors set in. In Sec. III we formulate the hodograph method and give general solutions of the hodograph equations, which then will be used to reveal features of the 2D current flows for particular geometries. In Sec. IV we consider current flow past a semi-infinite corner and calculate analytically the structure of the current domain walls and singularities in J(r) and E(r) distributions near sharp edges. In Sec. V we obtain a solution for current flow past a nonconducting planar defect in an infinite superconductor, and identify the new length scales of E(r) which are caused by the nonlinearity of E(J). We describe flux flow regions near the edge of the planar defect and address a nontrivial critical state limit at n→⬁. In Sec. VI we calculate excess dissipation on planar defects for nonlinear E(J) characteristics. Sec. VII is devoted to the discussion of the results and their implications for nonlinear current transport and current-limiting mechanisms in HTS’s. II. NONLINEAR 2D CURRENT FLOW A. Time scales In this paper we consider the 2D steady-state transport current flow, which sets in after initial relaxation of current distribution induced by switching on a dc power supply. In superconductors, such transient processes can dominate the 4007 observable behavior on ‘‘human’’ time scales, because the strong nonlinearity of J(E) can make the relaxation time t 0 astronomically large. In this case, the superconductor remains in a metastable critical state, which relaxes very slowly toward a true steady state. Therefore an estimation of t 0 is necessary to find the conditions, under which the steady-state current flow actually occurs. We estimate t 0 of macroscopic current relaxation, assuming that a superconductor is in a high magnetic field, so that both self-field effects and the surface or geometrical barriers can be neglected. In this case 0 H⫽B, and J(E,B) ⫽J(E,B 0 ), where B 0 / 0 is a constant applied magnetic field. Eqs. 共2兲 then reduce to 0 t E⫽⫺ⵜ⫻ⵜ⫻E. 共6兲 Here (E)⫽ J/ E is the differential conductivity, whose dependence on E⫽ 兩 E兩 determines the dynamics of E(r,t). The important feature of (E) in the subcritical state (E ⰆE c ) is an approximately inverse dependence (E) ⬇J 1 /E for all existing models of thermally activated vortex dynamics described by Eq. 共1兲.4 This universality holds in a very wide region of E to the accuracy of a much weaker logarithmic variation of J 1 (E) at large n⬃3 –30. Here the parameter J 1 ⫽T/ 兩 J U 兩 ⫽sJ can be expressed in terms of the observed dimensionless flux creep rate, s⫽d ln J/d ln t.1–4 Since macroscopic electrodynamics of superconductors becomes model independent, when formulated in terms of the electric field E(r,t), the time scale t 0 can be estimated by a scaling analysis of Eq. 共6兲.4 Indeed, Eq. 共6兲 can be regarded as a nonlinear diffusion equation for the electric field E with the diffusivity D(E)⫽1/ 0 . Thus the time scale t 0 of current redistribution in a region of size L is given by t 0 ⬃L 2 /D, whence t 0 ⬃ 0 L 2 J 1 /E. 共7兲 Here t 0 determines the duration of a transient process after which a steady-state current flow sets in. Because of the exponential dependence of E on J, the electric field E in Eq. 共7兲 共and thus t 0 ) can vary strongly within a superconductor. The upper bound of t 0 can be estimated by substituting the steady-state E(r) in Eq. 共7兲. For instance, taking the standard electric field criterion, E c ⯝1 V/cm for J c and a characteristic spacing between defects, L⯝100 m, we obtain t 0 ⯝0.06 sec, for J 1 ⫽sJ c , J c ⫽106 A/cm2 and s⫽0.05. In this case a steady-state transport current flow sets in on a short time scale, even for high J c values. However, geometrical constraints for certain sample geometries can make t 0 much larger than the above estimate. As an example, we first consider the current lead of width L 1 attached to a sample of width L 2 ⬎L 1 关Fig. 3共c兲兴, assuming the power law E⫽E c (J/J c ) n with n⯝3 –20. Let the lead be in a uniform critical state, (E 1 ⯝E c ), which sets in at t⬎t 1 ⯝ 0 sJ c L 21 /E c . Then it takes t⬎t 2 ⯝ 0 sJ c L 22 /E 2 for a steady-state uniform current flow to occur in the sample, where E 2 is determined by the current conservation condition, E 2 ⫽E 1 (L 1 /L 2 ) n , giving t 2 ⯝t 1 (L 2 /L 1 ) n⫹2 . For n ⫽15 and L 2 ⫽2L 1 , this yields t 2 ⯝1.3⫻105 t 1 , or about 2.2 h for t 1 ⫽0.06 sec. A similar argument can be made for the important case of a planar defect in a film 关Fig. 3共a兲兴, for which L 2 ⫽d, L 1 4008 ALEX GUREVICH AND MARK FRIESEN ⯝d⫺a, where d is the film thickness, and a is the length of the defect. If the electric field near defect is of order E c , then the electric field in the bulk, E 2 ⯝(1⫺a/d) n E 1 can be much smaller than E c , even for a small defect, aⰆd. Thus the steady-state current flow near defect sets in after t⬎t 1 ⯝ 0 sJ c (d⫺a) 2 /E c , while it can take a much longer time, t⬎t 2 ⬃t 1 /(1⫺a/d) n⫹2 in the bulk. For d⫽1 mm, n⫽15, J 1 ⫽5⫻104 A/cm2 , we find that t 1 ⯝6.3 sec, but t 2 ⬃38 sec for a⫽0.1d, t 2 ⬃45 min for a⫽0.3d, and t 2 ⬃9.6 days for a⫽0.5d. For larger a and n, relaxation toward a steady-state transport current distribution occurs on time scales well exceeding the experimental time window. The above examples show that, although the transient relaxation of J(r,t) could be very slow for certain geometries, the steady-state transport current flow for the most cases discussed in the Introduction sets in on rather short time scales. Such relaxation is accelerated in HTS’s, where flux creep is rather fast, and the n values are significantly smaller than in low-T c superconductors.3 In the rest of this paper we therefore consider the nonlinear steady-state 2D transport current flow in superconductors, disregarding the transient period t ⬍t 0 , on which steady-state E(x,y) is formed. The relevant time scales t 0 can be estimated from Eq. 共7兲 for any steadystate distribution E(x,y). B. Steady state For steady-state current flow, Eqs. 共2兲 become ⵜ⫻E⫽0, ⵜ⫻H⫽J. 共8兲 To satisfy the conditions div J⫽0 and ⵜ⫻E⫽0, for the 2D current flow in the xy plane, we introduce the scalar potential and the stream function , related to J and E as follows: J x⫽ y , E x ⫽⫺ x , J y ⫽⫺ x , 共9兲 E y ⫽⫺ y , 共10兲 where ␣ ⬅ / ␣ . The magnetic field H(r) is expressed in terms of (x ⬘ ,y ⬘ ) by the Bio-Savart law, H共 r兲 ⫽ 1 2 冕兵 V 共 r⫺r⬘ 兲 ⫻ 关 n̂⫻ⵜ ⬘ 兴 其 兩 r⫺r⬘ 兩 3 d 3 r⬘ , 共11兲 where the integral is taken over the current flow regions, and n̂ is the unit vector along the z axis. The stream function coincides with the normal component of the magnetic field H n for the 2D current flow in a long cylinder or slab, but can be very different from H n for thin films.27–31 For Ohmic conductors, both and satisfy the Laplace equation ⵜ 2 ⫽0, ⵜ 2 ⫽0, so it is convenient to introduce the complex potential w(z)⫽ ⫺i , which is an analytic function of the complex coordinate z⫽x⫹iy. Here ⫽E/J, and the real and imaginary parts of w(z) obey the boundary conditions for and ⫺ , respectively. This fact enables one to use powerful methods of the theory of analytic functions to calculate the 2D transport current flow in Ohmic conductors.32 This technique is also useful for calculation of magnetization currents in superconductors.27–29 PRB 62 In nonlinear conductors the situation is much more complicated, since w(z) is no longer analytic function. As a result, nonlinear current flow generally causes bulk charge density distribution, q⫽div E, q⫽ 共 J 兲 JⵜJ, 共12兲 since the resistivity ⫽E/J now depends on J. For instance, for the case shown in Fig. 3共c兲, integration of the charge density, q⫽div E, gives the total charge accumulated near the current injector, Q̄⫽(A 1 E 1 ⫺A 0 E 0 ). Here E 1 is the electric field in the injector, and E 0 is the electric field in the conductor, in regions far away from the joint, where both E 1 and E 0 are uniform, and A 1 and A 0 are the cross-sectional areas of the injector and the conductor, respectively. For uniform Ohmic conductors, the charge Q̄ vanishes because A 1 E 1 ⫽A 0 E 0 . By contrast, for nonlinear conductors and A 1 ⫽A 0 , we get Q̄⫽0, since A 1 E(I/A 1 )⫽A 0 E(I/A 0 ). The nonlinearity of E(J) gives rise to new length scales for the current distribution around a local inhomogeneity. To show that, we write Eq. 共4兲 in the form x xx ⫹ y y y ⫽0, 共13兲 where x ⫽ J x / E x and y ⫽ J y / E y are principal values of the differential conductivity tensor ik calculated from Eq. 共1兲: x ⫽ 共 J/E 兲 sin2 ⫹ cos2 , 共14兲 y ⫽ 共 J/E 兲 cos2 ⫹ sin2 . 共15兲 Here ⫽ J/ E is a scalar differential conductivity, and is the angle between the direction of the local electric field E(x,y) and the x axis, so that tan ⫽E y /E x . For isotropic Ohmic conductors, the conductivity tensor is also isotropic, ( x ⫽ y ), thus the electric-field perturbations, ␦ E(x,y), decay on a length scale of order the inhomogeneity size a, both along x and y. However, for any nonlinear isotropic E(J), not only does ik depend on E, it also becomes highly anisotropic with respect to the current flow ( x ⫽ y ). Assuming that far away from the inhomogeneity, the current streamlines are nearly parallel to the x axis ( Ⰶ1), we obtain that x ⯝ J/ E, and y ⯝J/E. In this case, the strong nonlinearity of E(J) in superconductors results in x Ⰶ y 关for the power-law E⫽E c (J/J c ) n , we have x ⫽ y /nⰆ y 兴. The relation x Ⰶ y reflects the fact that the longitudinal perturbations ␦ E x mostly change the modulus of J⬇J c , causing a rather weak current response ␦ J x ⫽( E J) ␦ E x . By contrast, the transverse perturbations ␦ E y cause a local turn of the vector Jc , resulting in a much larger current response ␦ J y ⯝(J c /E) ␦ E y . The fact that x Ⰶ y gives rise to a decay of E(x,y) perturbations over very different length scales L 储 and L⬜ along the x and y axes, respectively. As follows from Eq. 共13兲, we have L⬜ ⬃( y / x ) 1/2L 储 , whence L⬜ ⬃L 储 冑n. 共16兲 This relation will be illustrated below by exact solutions for particular current flows. Here we just give a simple physical estimate of L⬜ and L 储 for a planar defect of length 2aⰆd, as shown in Fig. 3共a兲. The defect blocks current flow on the PRB 62 NONLINEAR TRANSPORT CURRENT FLOW IN . . . 4009 length ⬃a, forcing the current aJ 0 to redistribute around the defect on the scale ⬃L⬜ . In the region y⬍L⬜ the mean current density and the electric field thus increase to J m ⬃(1⫹a/L⬜ )J 0 and E m ⬃(1⫹a/L⬜ ) n E 0 , respectively. The transverse decay length, L⬜ , is defined by the condition E m ⬃E 0 , giving L⬜ ⬃na. The decay length, L 储 ⬃a 冑n, along current flow then follows from Eq. 共16兲. Therefore strong (nⰇ1) nonlinearity of E(J) greatly increases the spatial scales of electric-field perturbations, as will be confirmed below by exact calculations. At the same time, E(x,y) can also vary on scales much smaller than a, as it occurs in narrow current domain walls, which replace the sharp d lines of the Bean model. In Eq. 共23兲 we can change variables, E⫽E c (J/J c ) n , and express as a function of E and , which is convenient for the further analysis of electric-field distributions. Equations 共23兲 and 共24兲 can also be presented in different useful forms by introducing new variables, III. HODOGRAPH TRANSFORMATION which has the form of the London equation with the inverse ‘‘screening length’’ ␤ : A. General formalism Instead of solving the nonlinear Eq. 共13兲, we change variables and take and to be functions of the complex electric field E x ⫹iE y ⫽E exp(i), where is the polar angle between E and the x axis. The advantage of such a hodograph transformation is that it reduces the highly nonlinear Eq. 共13兲 for (x,y) to linear equations for (E, ) and (E, ). To show this we write Eqs. 共8兲 in the differential form, d ⫽⫺E x dx⫺E y dy, d ⫽E y dx⫺E x dy, 共17兲 where (E)⫽E/J. Equations 共17兲 can be combined in a single complex equation d ⫺i d ⫽⫺Ee ⫺i dz, whence E z⫽⫺e i 共 E ⫺i E 兲 /E, i z⫽⫺e 共 ⫺i 兲 /E. 共18兲 共19兲 Here z⫽x⫹iy is the complex coordinate, and (E) ⫽ J/ E is the differential conductivity 共notice that in nonlinear conductors ⫽1/ ). The condition 2 E z⫽ E2 z then gives the following relations between partial derivatives of and : ⫽⫺ 共 E 2 /J 兲 E , E ⫽ 共 E /J 2 兲 . 共20兲 Equating the mixed derivatives, 2 E ⫽ E2 , for and , we obtain the following linear equations for and valid for any nonlinear dependence J(E): E 2 J2 J 2 E2 ⫹ 2 冉 冊 冉 冊 E2 ⫽0, E J E 共21兲 J 2 ⫽0. E E E 共22兲 ⫹ 2 ⫽e ␤ h 1 , ⫽e ⫺ ␤ h 2 , ⫽ 1 冑n ln E . E0 共25兲 Here E 0 is the electric field at infinity, and the functions h 1,2( , ) satisfy the equation, 2 2 h⫹ h⫺ ␤ 2 h⫽0, ␤ ⫽ 共 n⫺1 兲 /2冑n. 共26兲 共27兲 Therefore the nonlinearity of E(J) results in an effective screening of ( , ) in the hodograph space, which becomes stronger as n increases. For n⫽1, Eq. 共26兲 turns into the Laplace equation, thus the complex potential w(u)⫽ ⫺i is an analytic function of u⫽ ⫺i in the hodograph representation. Analytic properties of the complex potential w( , ) in nonlinear conductors are considered in Appendix A. We show that for n⬎1, w( , ) is no longer analytic function, but can be expressed in terms of generalized analytic functions.33 B. Solving the hodograph equations The calculation of nonlinear current flow by the hodograph method is implemented in two steps. First, a solution of the linear Eq. 共21兲 should be found, which satisfies the particular boundary conditions. Then an inverse transformation of ( ,E) from the hodograph plane (E, ) onto the physical xy plane should be performed to obtain the current streamlines ⫽ (x,y) and spatial distributions of the electric fields and currents. As shown in Appendix E, the Jacobian of the inverse transformation does not change sign for any isotropic E-J characteristic with positive differential conductivity (E).21 This fact makes the hodograph transformation a well-defined procedure, for which each solution (E, ) corresponds to a unique spatial distribution of E(x,y) for given boundary conditions. Solutions of Eqs. 共21兲 and 共22兲 can be obtained by separating variables as follows: 共 E, 兲 ⫽ 兺 C m f m 共 E 兲 sin共 m ⫹ m 兲 . m 共28兲 For the power-law dependence, E⫽E c (J/J c ) n , these equations simplify to Here C m and m are constants, and the functions f m (E) satisfy the following ordinary differential equation: 2 J 2 2 ⫹ ⫹J ⫽0, n J2 J 2 共23兲 m 2 E d E2 d f m ⫺ f m ⫽0. dE J dE J2 共24兲 An analogous expression to Eq. 共28兲 for the electric potential (E, ) can be obtained with the eigenfunctions g m (E) satisfying 2 nE ⫹ ⫹E ⫽0. E 2 E2 2 2 冉 冊 共29兲 4010 ALEX GUREVICH AND MARK FRIESEN 冉 冊 d J 2 dg m m 2J ⫺ 2 g m ⫽0. dE E dE E 共30兲 For the power-law J(E) characteristic, Eq. 共23兲 gives f m (E)⬀E q m , so (E, ) takes the form z⫽z ⫾ ⫹e i e i ⫺ J 冉 PRB 62 B 1 B 2E 0 ⫹ 关 1⫹i 共 n⫺1 兲共 ⫹ 0 兲兴 J nE ⬁ 兺 m⫽0 冉 冊 ⫾ Cm E ⫾ nq m ⫺1 E 0 冊 ⫾ qm ⫾ sin m 兲 . 共 m cos m ⫺inq m 共36兲 共 E, 兲 ⫽ 0 ⫹ 关 B 1 ⫹B 2 共 E/E 0 兲 1/n⫺1 兴共 ⫹ 0 兲 ⫹ ⫾ ⫽ qm 兺m ⫾ Cm 冉 冊 E E0 ⫾ qm sin共 m ⫹ m 兲 , 1 关 1⫺n⫾ 冑共 n⫺1 兲 2 ⫹4nm 2 兴 . 2n 共31兲 共32兲 Here the sum runs over all integer m, the constants B 1,2 , ⫾ , 0 , 0 , E 0 , and m are determined by the boundary Cm conditions, and E 0 can be taken as the electric field at infinity. We emphasize that Eqs. 共31兲 and 共32兲 are exact general solutions of the nonlinear Maxwell equations which describe various current flows. If distributions E(x,y) contain regions of E⬍E 0 and E (⫹) (⫹) (⫺) (⫺) , qm , and C m , qm , the ⬎E 0 , with different sets of C m solutions ⫹ (E, ) for E⬎E 0 and ⫺ (E, ) for E⬍E 0 should be matched at E⫽E 0 as to provide continuity of (E, ) and its derivatives. Finding the proper relation be(⫹) (⫺) and C m can be reduced to the solution of the tween C m following linear matrix equation:25 兺k U mk C k ⫽F m , 共33兲 where U mk and F m are determined by the sample geometry. The fact that both ⫺ (E, ) and ⫹ (E, ) are known exactly is a great advantage of the hodograph method, which thus reduces the initial nonlinear problem to a standard procedure of matrix inversion. In some cases the coefficients C m can be ⫺1 F k can be efobtained analytically, otherwise C m ⫽ 兺 k U km 25 fectively calculated numerically. Since the hodograph method linearizes the Maxwell equations for any E(J), numerical calculations of nonlinear current flow J(x,y) for the cases shown in Figs. 2 and 3 take no longer than the corresponding calculations of J(x,y) for Ohmic conductors. The solution 共31兲 is rather convenient for performing the inverse transformation of (E, ) onto the coordinate space xy, giving the electric-field distribution z⫽z(E, ) for any ⫾ . This is a well-defined mathematical procedure, set of C m since the Jacobian of the inverse transformation is always positive for any isotropic E-J characteristic, as shown in Appendix E. To obtain E(x,y), we exclude E and from Eqs. 共20兲, which yields z⫽ E z⫽ e i 共 E E ⫹i 兲 , J 冉 冊 e i i E ⫺ . J J ⫾ , and the plus and the Here z ⫾ are constants, m ⫽m ⫹ m minus signs correspond to E⬍E 0 and E⬎E 0 , respectively. Equations 共36兲 represent a complete family of exact solutions of nonlinear Maxwell’s equations for various distributions E(x,y), parameterized by an infinite set of constants C m . In the following sections we will show how C m can be found for particular current flows. Equation 共26兲 belongs to the well-studied linear equation of mathematical physics, so various nonlinear current distributions can be obtained from known solutions for other physical problems described by the London or diffusion equations. For instance, a solution ( , ) of Eq. 共23兲 inside the region bound by the contour S in the hodograph plane can be expressed in terms of the surface distribution b (s): 共 , 兲 ⫽e ⫺ ␤ 冖 S e ␤ ⬘ b 共 s 兲 n G 共 , ⬘ , , ⬘ 兲 ds. 共37兲 Here ( , ) is determined by the boundary conditions, the Green’s function G of Eq. 共26兲 satisfies the boundary condition G⫽0 on S, and n denotes the normal derivative on S. The function G has a clear physical meaning, since it is proportional to the local magnetic field at the point , produced by a fictitious London vortex located at the point ⬘ , ⬘ in a superconducting cylinder. This analogy enables one to use extensive results on vortices in superconductors of different geometries to calculate G( , ⬘ , , ⬘ ) and thus 2D current flows in nonlinear conductors.22 Another analogy follows from the following representation of Eqs. 共23兲 and 共24兲: 2 2 ⫹ ⫹2 ␤ ⫽0, 共38兲 2 2 ⫹ ⫺2 ␤ ⫽0. 共39兲 Equations 共38兲 and 共39兲 have the form of diffusion equations, which describe steady-state distributions of the fields or in a reference frame moving with the velocity ⫾2 ␤ . Equations 共38兲 and 共39兲 also belong to the well-studied linear equations,34 which could help on finding solutions of the hodograph equations, using the known solutions of the corresponding diffusion problems. For instance, in the critical state limit (n→⬁), Eq. 共23兲 becomes a simple 1D diffusion equation in the hodograph space 共34兲 ⫽ , 共35兲 where ⫽ln(Jc /J) and play the roles of ‘‘time’’ and ‘‘coordinate,’’ respectively. In this case the solution of Eq. 共40兲 for the stream function Substituting Eq. 共31兲 into Eq. 共35兲 and integrating over E, we obtain ⬁ ⫽B ⫹ 兺 C m m⫽1 冉冊 J Jc 共40兲 m2 sin共 m ⫹ m 兲 共41兲 NONLINEAR TRANSPORT CURRENT FLOW IN . . . PRB 62 4011 flow inside or outside of two unpenetrable walls inclined at the angle ␣ 共Fig. 5兲. This case allows us to calculate structure of the current domain walls and trace the nonanalytic crossover from large, but finite n value, to the critical state limit n→⬁. A. General solution The solution for current flow around the corner, satisfies the boundary conditions, (E,0)⫽ (E, ␣ )⫽0, corresponding to zero normal component of J on the sample surface. This solution of Eq. 共23兲 has the form ⫽CE q sin k , 共42兲 where k⫽ /( ⫺ ␣ ), C is a scaling constant, and FIG. 5. Inner 共a兲 and outer 共b兲 current flows around a corner. is independent of n and therefore can be regarded as a ‘‘critical state’’ limit for (J, ). However, as will be shown below, Eq. 共41兲 can result in current distributions, which are different from those of the Bean model. C. Boundary conditions To take advantage of the exact solutions for (E, ) and (E, ), we need to reformulate the corresponding boundary conditions in the hodograph space. This procedure is rather nontrivial, since even simple boundary conditions in the xy plane, such as zero normal component of J on the sample surface, or a given distribution of J or E on the electrodes, can become highly nonlinear in the E plane. For instance, if current flows past a cylindrical void of radius R, the condition of zero normal component of J(x,y) requires constant (x,y)⫽ 0 on the surface, x 2 ⫹y 2 ⫽R 2 . Taking the hodograph solutions x⫽A(E, ),y⫽B(E, ), we obtain the boundary conditions in the E plane: A 2 (E, )⫹B 2 (E, ) ⫽R 2 and (E, )⫽ 0 . Substituting here Eq. 共36兲, we arrive at an infinite set of coupled nonlinear equations for C m and m . Therefore the boundary conditions become nonlinear for curved boundaries or nonuniform distributions of J(x,y) on the electrodes. However, for any 2D current flow confined between flat, piece-wise boundaries, or around planar cuts 共see Figs. 2 and 3兲, the boundary conditions in the hodograph space greatly simplify. Then the condition of zero normal component of J at the straight boundary inclined by the angle 0 becomes linear, reducing to (E, 0 )⫽ 0 , where 0 is a constant. For example, for current flow around a corner shown in Fig. 5, the boundary conditions can be taken in the form, (E,0) ⫽ (E, ␣ )⫽0. Therefore, for current flow around planar obstacles, the hodograph transformation linearizes both the equation for (E, ) and the boundary conditions. In this case we can obtain complete exact solutions of the nonlinear Maxwell equations considered in the following sections. IV. CORNER One of the simplest exact solutions of Eq. 共23兲 describes current flow around a corner. There are two different situations which we consider separately, corresponding to current 1 关 1⫺n⫾ 冑共 1⫺n 兲 2 ⫹4nk 2 兴 . 2n q⫾ k ⫽ 共43兲 Here the plus and the minus signs correspond to current flow inside and outside the region of the angle ␣ , respectively 共Fig. 5兲. Taking the origin, z⫽0, as the vertex for both cases, we obtain the distribution of E(x,y), substituting Eq. 共42兲 into Eq. 共35兲 and integrating from 0 to E for q⫽q ⫹ and from ⬁ to E for q⫽q ⫺ . This yields z⫽⫺ Ce i E q 共 k cos k ⫺iqn sin k 兲 . 共 qn⫺1 兲 J 共 E 兲 共44兲 Separating real and imaginary parts of Eq. 共44兲, and excluding E by dividing y(E, ) by x(E, ), we obtain the following equation for the function (x,y), which determines local orientation of current flow y k tan ⫺nq k tan k . ⫽ x k⫹nq k tan tan k 共45兲 We use these results to consider two particular cases: 共i兲 Current flow past a semi-infinite cut, for which q⫽⫺1, ␣ →0; 共ii兲 Current flow near a rectangular corner, for which q⫽q ⫾ 2 , ␣ ⫽ /2. In the first case, ⫽C sin /E is independent of n, and Eq. 共44兲 gives z⫽ Ce i 共 cos ⫹in sin 兲 . 共 n⫹1 兲 JE 共46兲 Current streamlines described by Eqs. 共42兲 and 共46兲 are shown in Fig. 6. For nⰇ1, current streamlines are approximately semicircles centered near the end of the cut, while contours of constant electric field are close to circles which cross the cut. Near the edge, (x⬇0,y⫽0), the electric field E(x) has a singularity. For x⬍0 and y→⫾0, currents flow parallel to the cut 关 ⫽0 at y⫽⫹0, or ⫽ at y⫽⫺0, 共see Fig. 6兲兴, and Eq. 共46兲 gives x⫽C/(n⫹1)JE. For x⬎0, we have ⫽ /2, and x⫽⫺nC/(n⫹1)JE, whence E 共 x 兲 ⬀1/nx n/(n⫹1) , x⬍0, 共47兲 E 共 x 兲 ⬀1/x n/(n⫹1) , x⬎0. 共48兲 Hence the circle of constant E of radius R crosses the cut at the point ⯝R/n away from the edge. For the linear case, n ⫽1, Eq. 共48兲 gives the square-root singularity J(x) 4012 ALEX GUREVICH AND MARK FRIESEN FIG. 6. Nonlinear current flow around a semi-infinite cut. Dashed circle shows a contour of constant electric field. For n →⬁, all circular contours of constant E touch the end of the cut. PRB 62 FIG. 8. Nonlinear current flow around a corner. For nⰇ1, current streamlines in the upper right quadrant are nearly circular, and centered in the vertex. ⫽E(x)⬀1/兩 x 兩 1/2, both in J(x) and E(x) at 兩 x 兩 →0.24,32 For nⰇ1, the nonlinearity of J(E) in superconductors enhances the singularity in E(x)⬀1/兩 x 兩 , while strongly suppressing the singularity in J(x)⬀1/兩 x 兩 1/n . For the semiconductor-type nonlinearity, nⰆ1, the situation is the opposite: the singularity in E(x) is suppressed, but enhanced in J(x). The second example is the rectangular corner shown in Figs. 7 and 8. There are two different cases of current flow inside and outside the corner, which correspond to q⫽q ⫹ 2 ⬎0 and q⫽q ⫺ 2 ⬍0 in Eq. 共42兲, respectively. Excluding E from Eqs. 共42兲 and Eq. 共44兲, we obtain the current streamlines x⫽Re z( , ) and y⫽ Im z( , ) in the form22 冉 冊 z⫽D sin 2 ⫹ FIG. 7. Current flow near the corner of a rectangular sample for a superconductor (n⫽50) 共a兲 and a normal metal 共b兲. The dashed straight lines in 共a兲 show boundaries of a diverging current domain wall, defined as a region where 兩 ⫺ /4兩 ⬍0.3. ⫹ 1⫺1/nq 2 i 共 2 cos 2 ⫺inq ⫹ 2 sin 2 兲 e , 共49兲 ⫹ where D⫽C 1/nq 2 E 1/n 0 /J 0 (nq 2 ⫺1). Each streamline corresponds to a contour of constant . The evolution of the current distribution with n is shown in Fig. 7. For n⫽1, we have q⫹ 2 ⫽2, thus Eq. 共49兲 gives smooth hyperbolic streamlines, ⬀xy.24,32 By contrast, the highly nonlinear case nⰇ1 exhibits sharp changes of the current flow direction near the diagonal somewhat reminiscent of, yet different from the piece-wise current distribution of the Bean model 共see below兲. Current flow past the corner in Fig. 8 exhibits quite different characteristics which manifest themselves in the distribution of local orientations, (x,y). For nⰇ1 Eq. 共43兲 2 gives nq ⫺ k ⬇⫺(n⫹k ⫺1), thus Eq. 共45兲 simplifies to x/y ⫽⫺tan . The relation x/y⫽⫺tan describes circular current streamlines centered in the vertex and is valid everywhere, except for narrow regions of angles, ␦ ⯝n ⫺1/2, near ⫽0 and ⫽ ⫺ ␣ , which correspond to currents flowing almost parallel to the sample surface. Therefore current flow around the semi-infinite corner described by exact Eq. 共45兲 exhibits no trace of singular d lines characteristic of the case shown in Fig. 7共a兲. The solutions of this subsection contain a scaling constant C, which remains undetermined for semi-infinite samples. If the corner is a part of a defect in a finite sample, say, a PRB 62 NONLINEAR TRANSPORT CURRENT FLOW IN . . . 4013 surface notch or a step in a film, the above solutions describe current flow only near the corner. The constant C is determined by current distribution far away from the defect and thus depends on the sample geometry and the boundary conditions 共see below兲. Here we just note that the particular value of C does not affect the shape of the current stream lines described by the function (x,y). This fact enables us to investigate universal features of the current domain walls, based on the exact, yet simple solutions 共42兲–共45兲, regardless of the particular geometry of the whole sample. B. Structure of the current domain wall The principal question is how the singular d line emerges in a smooth current distribution as n→⬁. For the Bean model, the d line manifests itself in a step-wise change of the current orientation, (x,y)⫽ 关 sgn(x⫺y)⫺1 兴 /4, as seen in Fig. 4共a兲. Although such a step-wise current configuration satisfies the critical state assumption, J⫽J c , and the continuity of the normal component of J, it has a jump of tangential component J 储 along the d line. Thus this model distribution of J(x,y) cannot exist in steady state, if any electric field caused by current flow is taken into account. Indeed, a jump in J 储 on the d line would result in a discontinuity of the tangential component of E, which violates ⵜ⫻E⫽0. For finite nⰇ1 this discontinuity is smoothed out, and the d line turns into a current domain wall of finite thickness between regions with different orientations of current flow, as follows from extensive numerical simulations performed by Brandt.17 Here we address the following questions, which are rather difficult to resolve through numerical simulations: 共i兲 Is there any intrinsic width of the current domain wall, which is determined by the nonlinearity of J(E) regardless of the sample geometry? 共ii兲 Is there an analytic crossover from large, but finite n to the Bean model behavior at n →⬁? 共iii兲 Is the d line of the Bean model a true steady state in the limit n→⬁? 共iv兲 Is there any singularity in current domain wall in the limit n→⬁? The exact hodograph solutions show that only the last proposition is true, while the very existence of the d line depends on the geometry of current flow. For example, the Bean model predicts the d lines for current flow both inside and outside a corner, depending on the magnetic prehistory. The results of the previous subsection indicate that, although some sort of singularity on the diagonal remains for the inside flow in Fig. 7共a兲, the outside flow in Fig. 8 always exhibits nonsingular circular streamlines. The latter solution also satisfies the Bean model. Therefore we see that even exponentially weak electric field in the critical state (nⰇ1) drives the step-wise current distribution in Fig. 4共a兲 into the nonsingular one in Fig. 7共a兲, corresponding to the true steady state. We now consider the structure of the current domain wall in Fig. 7共a兲 in more detail by analyzing the behavior of the function (x,y) near the diagonal, where x⬇y, ⫽⫺ /4 2 2 2 ⫹ ␦ , and ␦ Ⰶ1. If nⰇ1, we have nq ⫹ k ⬇k ⫺k (k ⫺1)/n, so Eq. 共45兲 for ␦ Ⰶ1, simplifies to 冉 冊 3 x⫺y ⫽2 ␦ ⫹ ␦ 2 . x n 共50兲 FIG. 9. Structure of the current domain wall for different n values. The dashed line shows the step-wise dependence ␦ (x,y) of the Bean model. From Eq. 共50兲 it follows that there is no ‘‘intrinsic’’ width of the current domain wall, since ␦ (x,y) is a power-law function of x and y near the diagonal. If we define the domain wall as a region, in which ␦ ⬍ ␦ 0 , then Eq. 共50兲 gives its width, d(l 储 , ␦ 0 ), as a function of the conditional criterion ␦ 0 and the distance l 储 ⫽(x⫹y)/2 from the vertex along the diagonal. We thus obtain that the so-defined width of the current domain wall, d⫽ ␦ 0 (3/n⫹ ␦ 20 )l 储 linearly increases with l 储 and remains finite even in the limit n→⬁. The dependence of (l 储 ,l⬜ ) on the coordinate l⬜ ⫽(x⫺y)/2 across the d line at a fixed distance l 储 from the vertex is shown in Fig. 9. For finite n, we obtain that ␦ ⫽nl⬜ /3l 储 is linear when l⬜ Ⰶl 储 (3/n) 3/2 and acquires the universal dependence ␦ ⫽(l⬜ /l 储 ) 1/3 when l⬜ Ⰷl 储 (3/n) 3/2 . Therefore the exact theory predicts continuous broadening of the d line with l 储 , as observed in magneto-optical experiments.7 In the limit n→⬁, we have ␦ ⫽(l⬜ /l 储 ) 1/3 for all l⬜ , thus the function (l⬜ ) remains continuous at l⬜ ⫽0, but the derivative / l⬜ ⬀l⬜⫺2/3 diverges, in stark contrast to the jump in (x,y) for the Bean model. Such a ‘‘soft’’ singularity in (x,y) is rather difficult to reveal in numerical simulations of nonlinear Maxwell’s equations in the coordinate space. Therefore, for n→⬁, some kind of singular d lines do appear, but the behavior of (l 储 ,l⬜ ) turns out to be quite different from the Bean model 共see Fig. 9兲. This difference is due to the fact that the hodograph solutions satisfy the condition ⵜ⫻E⫽0, even for n→⬁. V. PLANAR DEFECT IN AN INFINITE SUPERCONDUCTOR Now we consider a more complicated problem of current flow past a thin nonconducting planar defect of length 2a in an infinite media 共Fig. 10兲. This case models the strongest current-limiting defects in HTS’s, such as high-angle grain ALEX GUREVICH AND MARK FRIESEN 4014 PRB 62 weak. In this case it is convenient to write Eq. 共26兲 in polar coordinates (r, ), with the origin at the end of the cut, ⫽0, ⫽ /2: rr h⫹r ⫺1 r h⫹r ⫺2 h⫺ ␤ 2 h⫽0, 共53兲 where ⫽r cos , ⫽ /2⫹r sin , and ␤ is given by Eq. 共27兲. If ␤ →⬁, the function h(r, ) describes a vortex at the end of the cut in an infinite media. In this case, an exact vortex solution of Eq. 共53兲 is h⫽ 冑2h 0 FIG. 10. Mapping of the current flow around a thin nonconducting strip in the xy plane 共inset兲 onto the hodograph plane . boundaries, or microcracks. To capture the general features of ( , ), we first consider the complex potential w(z) for the same geometry in the case of Ohmic conductors,24 w⫽iE 0 冑z 2 ⫺a 2 . 共51兲 Expressing w via the complex electric field, E exp(⫺ı)⫽ ⫺dw/dz 共see Appendix A兲, we obtain w⫽⫺ aE 0 冑1⫹exp 2 共 ⫺i 兲 , 共52兲 where ⫽ln(E/E0). As follows from Eq. 共52兲, the stream function ⫽Im(w) has a singularity at ⫽0, ⫽ /2 and decays exponentially away from this point, on the scale ⬃1, ⫺ /2⬃1. The boundary conditions for ( , ) in the hodograph plane follow from the symmetry properties of the current flow around the defect 共Fig. 10兲. First, we notice that the zero x component of J on the central line 共perpendicular to the defect兲 requires the boundary condition ( , /2)⫽0. Along the ray x⫽0,⫺⬁⬍y⬍0, the electric field varies from its value at infinity, E⫽E 0 , to zero at the stagnation point, z⫽0, in the center of the planar defect. Furthermore, the zero normal component of J on the defect surface also requires ( ,0)⫽ ( , )⫽0, with E changing from 0 at z⫽0 to infinity at the edges (z⫽⫾a). In the hodograph plane ( , ), these boundary conditions give ⫽0 along two vertical lines at ⫽0 and ⫽ and along the half-infinite line ⫺⬁⬍ ⬍0 at ⫽ /2 共Fig. 10兲. Along the ray, ⬎0, ⫽ /2, we have ⫽0. Therefore the problem reduces to the solution of the London Eq. 共26兲 that describes a ‘‘vortex’’ at the end of the half-infinite cut, in the center of a superconducting film of thickness . The nonlinearity results in effective ‘‘screening’’ in Eq. 共26兲, making h( , ) more localized near the end of the cut in Fig. 10. For nⰇ1, h( , ) decays exponentially over the scale ⬃1/␤ Ⰶ1, so the influence of the boundary conditions on h( , ) at ⫽0, becomes very e ⫺␤r cos . 2 冑r 共54兲 Solutions with higher order harmonics ⬀ cos m/2, give unphysical distributions J(x,y), which we do not consider here. To satisfy the boundary condition ⫽0 at ⫽0, , for finite ␤ , we use the method of images, by presenting as a superposition of the fields of alternating vortices and antivortices at ⫽0, ⫽ m ⫽ (m⫹1/2), where m⫽0,⫾1, . . . . This yields ⫽h 0 兺 共 ⫺1 兲 m 冑r m ⫹ rm m e ⫺ ␤ (r m ⫹ ) , 共55兲 where r m ⫽ 冑 2 ⫹( ⫺ m ) 2 , and h 0 is a scaling constant, which will be obtained below. For nⰇ1, the sum in Eq. 共55兲 converges very rapidly, since exp(⫺␤)Ⰶ1, thus we can retain only nearest neighbors (m⫽0,⫾1). Now we come back to the general Eq. 共31兲, in which B 1,2⫽ m ⫽0 by symmetry, and C m are just the Fourier coefficients of the function (E 0 , ): C m⫽ 4 冕 /2 0 共 E 0 , 兲 sin m d . 共56兲 For nⰇ1, (E 0 , ) is localized around ⫽ /2, so we extend the upper limit in Eq. 共56兲 to infinity and retain only the term with m⫽0 in Eq. 共55兲. Then (E 0 , ) ⫽h 0 exp(⫺␤兩⫺/2兩 )/ 冑兩 ⫺ /2兩 , and Eq. 共56兲 gives C m ⫽(4h 0 / 冑 )Im关 exp(im/2)/ 冑␤ ⫺im 兴 , whence C 2k ⫽h 0 C 2k⫺1 ⫽h 0 2 3/2共 ⫺1 兲 k 冑 ␣ 2k 2 3/2共 ⫺1 兲 k 冑 ␣ 2k⫺1 冑␣ 2k ⫺ ␤ , 共57兲 冑␣ 2k⫺1 ⫹ ␤ , 共58兲 where ␣ m ⫽ 冑␤ 2 ⫹m 2 , and k is any integer. To satisfy the boundary condition ( , /2)⫽0 for E⬍E 0 , we take m ⫽2k in Eq. 共31兲. For E⬎E 0 , we have / ⫽0 at ⫽ /2, hence m⫽2k⫺1. As a result, Eq. 共31兲 can be presented in the form ⬁ ⫽ 兺 C 2k k⫽1 冉 冊 E E0 ⫹ q 2k sin 2k , E⬍E 0 , 共59兲 NONLINEAR TRANSPORT CURRENT FLOW IN . . . PRB 62 ⬁ ⫽ 兺 C 2k⫺1 k⫽1 冉 冊 E0 E 4015 ⫺ 兩 q 2k⫺1 兩 sin共 2k⫺1 兲 , E⬎E 0 . 共60兲 To transform (E, ) back onto the xy plane, we substitute Eqs. 共59兲 and 共60兲 into Eq. 共35兲. Since E⫽0 at z⫽0, we obtain z(E, ) in the region of E⬍E 0 , integrating Eqs. 共35兲 over E from 0 to E: z⫽⫺ ⬁ e i J0 兺 k⫽1 C 2k 冉 冊 E ⫹ nq 2k ⫺1 E 0 ⫹ q 2k ⫺1/n ⫹ ⫻ 关 2k cos 2k ⫺inq 2k sin 2k 兴 , E⬍E 0 . 共61兲 In the region where E⬎E 0 , we use the fact that E⫽⬁ at z ⫽a. Substituting Eq. 共60兲 into Eq. 共35兲 and integrating over E from ⬁ to E, we obtain for E⬎E 0 : e i z⫽a⫹ J0 ⬁ 兺 k⫽1 冉 冊 C 2k⫺1 E0 n 兩 q 2k⫺1 兩 ⫹1 E ⫺ 兩 q 2k⫺1 兩 ⫹1/n ⫻ 关共 2k⫺1 兲 cos共 2k⫺1 兲 ⫹in 兩 q 2k⫺1 兩 sin共 2k⫺1 兲 兴 . 共62兲 The constant h 0 calculated in Appendix B is determined by the self-consistency condition z(⫹0,0)⫽z(⫺0,0), which gives for nⰇ1 h 0 ⫽J 0 an 3/4/ 冑2 . 共63兲 The current flow described by Eqs. 共59兲–共63兲 is very different from that of Ohmic conductors 共Fig. 11兲.35 The most visible manifestation of nonlinearity is the long-range disturbance of current streamlines on the scales much larger than the defect size, 2a. If n→⬁, the magnitude of J(x,y)⫽J c remains approximately constant everywhere, but a region near the central line, x⫽0. In addition, the vector J changes the direction at diverging current domain walls, reminiscent of the d lines for magnetization current flow past a cylindrical hole in the Bean model 共Fig. 4兲. For finite n, the width of the current domain walls increases as the distance from the strip increases, providing the decay of current perturbations on the scale L⬜ Ⰷa. Spatial scales of nonlinear current flow around the strip can be obtained by considering electric-field distributions along two symmetry lines: in the plane of the defect (y ⫽0, x⬎a, ⫽ /2), and along the central line (x⫽0, y ⬍0, ⫽ /2). In the first case, substituting Eq. 共55兲 into Eq. 共35兲 at ⫽ /2, we obtain after integration over E: 冋 冉 冊册 冑 E E0 x⫺a erfc ln1/2 ⫽ ⫺ 1/2 L⬜ n E 0 E ln 共 E/E 0 兲 L⬜ ⫽ 冑2h 0 n 1/4/J 0 ⫽an/ 冑 . , 共64兲 共65兲 For nⰇ1, the last term in Eq. 共64兲 关proportional to the error function erfc(x)兴 can be neglected. As shown in Appendix C, Eq. 共64兲 is valid everywhere, except the very narrow vicinity of the defect edge x⫺a⬍a 冑n exp(⫺n/8), where E→⬁. In FIG. 11. Current flow around a planar defect 共only one quadrant is shown兲. 共a兲 corresponds to a superconductor described by Eqs. 共59兲–共63兲, where dashed contours show extended regions of enhanced (E⬎1.5E 0 ) and reduced (E⬍E 0 /2) electric field. 共b兲 shows current flow around the planar defect in Ohmic conductors, where perturbations of J(x,y) and E(x,y) decay on the length ⬃a. this region we can retain only one term, k⫽1, with the ⫺ 兩 ⫹1/n in the exact expansion 共62兲. smallest exponent 兩 q 2k⫺1 For nⰇ1, this yields E 0x ⫾ E 共 x,0兲 ⬇ , 兩 x⫺a 兩 J 共 x,0兲 ⫽J 0 冉 冊 x⫾ 兩 x⫺a 兩 1/n , 共66兲 where x ⫹ ⫽ 兩 C 1 兩 /J 0 ⫽4a 冑n/ for x⬎a, and x ⫺ ⫽ 兩 C 1 兩 /nJ 0 ⫽4a/ 冑n for x⬍a. Thus the nonlinearity of E(J) strongly ALEX GUREVICH AND MARK FRIESEN 4016 FIG. 12. Distributions of E y (x) in the plane of the defect (y ⫽0), described by Eq. 共64兲 for nⰇ1, and by Eq. 共67兲 for n⫽1. For x⫺aⰆa, the curves have the slopes ⫺1 for nⰇ1 and ⫺1/2 for n ⫽1, because near the edge of the defect, E⬀ 兩 x⫺a 兩 ⫺1 and E ⬀ 兩 x⫺a 兩 ⫺1/2 for superconductors and normal metals, respectively. The kink in ln(E/E0⫺1) at E⬃E 0 corresponds to a crossover to the large-x asymptotics: E⫺E 0 ⬃nE 0 (a/x) 2 at x⬃L⬜ . suppresses the singularity in J(x), while enhancing the singularity in E(x) at x⫽a, as compared to the Ohmic case, for which24 E 共 x,0兲 ⫽ E 0x 冑x 2 ⫺a 2 , 共67兲 n⫽1, x⬎a. Several important results follow from Eqs. 共64兲 and 共65兲, as shown in Fig. 12. First, the nonlinearity of E(J) considerably enhances a characteristic magnitude E m of the electric field. Since E⬃anE 0 /(x⫺a) over a wide region, x⬍L⬜ , near defect, we have E m ⬃nE 0 ⰇE 0 , L⬜ ⬃naⰇa. PRB 62 FIG. 13. Distribution of E(y) along the central line, x⫽0, described by Eq. 共69兲 for nⰇ1 and by Eq. 共70兲 for n⫽1. The length L 储 of a region of suppressed E(y) scales as a 冑n. E 共 0,y 兲 ⫽ E 0兩 y 兩 冑a 2 ⫹y 2 , n⫽1. 共70兲 For n⫽1, both E(0,y)⬀ 兩 y 兩 and J(0,y)⬀ 兩 y 兩 decrease linearly near the stagnation point y⫽0, restoring their background values E 0 and J 0 on the scale y⯝a. By contrast, for nⰇ1, we observe a long-range depression of E(0,y) on a scale L 储 Ⰷa, and a cusp in J(0,y) 共Figs. 13 and 14兲. The behavior of E(0,y) and J(0,y) at yⰆa can be obtained by taking the term with the minimum exponent with k⫽1 in Eq. 共69兲, which yields for nⰇ1 共68兲 Equation 共64兲 predicts a rather slow hyperbolic dependence of E(x,0) with no definite length scales, so the estimate 共68兲 only gives a characteristic mean value of E(x,0) in the region x⬃L⬜ , where E m ⰇE 0 . Here L⬜ quantifies a distance from the defect where E(x,0)⯝anE 0 /x becomes of the order of the background electric field E 0 . For larger distances, x⬎L⬜ , the parabolic dependence E(x,0)⬀1/(x⫺a) gradually turns into a more rapid decay, E(x,0)⫺E 0 ⬃(an/x) 2 E 0 for xⰇL⬜ 共Fig. 12兲. Distributions of E(0,y) and J(0,y) along the central line (x⫽0) are also strongly affected by the nonlinearity 共Fig. 13兲. To calculate E(y), we set ⫽ /2 in Eq. 共61兲 and obtain ⬁ 兩 y 兩 ⫽y 0 兺 k⫽1 k 冑␣ 2k ⫺ ␤ 冉 冊 E ␣ 2k 共 ␣ 2k ⫺ ␤ ⫺n ⫺1/2 兲 E 0 ␣ 2k ⫺ ␤ / 冑n⫺1/n , 共69兲 where y 0 ⫽2 5/2h 0 / 冑 nJ 0 ⫽4an 1/4/ . The dependence E(0,y) for nⰇ1 is rather different from that for Ohmic conductors, FIG. 14. Distribution of J(y) along the central line, x⫽0, described by Eq. 共86兲 for n→⬁ and by Eq. 共82兲 for n⫽1. NONLINEAR TRANSPORT CURRENT FLOW IN . . . PRB 62 4017 A. Local flux flow near sharp edges The above solutions, obtained for the power-law E(J), exhibit singularities of the electric field E(x)⬀1/(x⫺a) near the edges of planar defects. Such a strong enhancement of E(x) indicates that local flux flow can be induced near the edges, even though the E 0 away from the defect is much smaller than the crossover electric field E c between flux flow and flux creep regimes. Description of the current flow near the edges requires accounting for the full nonlinear dependence E(J). First we consider current flow near a half infinite cut, for which the solution of the hodograph Eq. 共21兲 should satisfy the boundary conditions (E,0)⫽ (E, )⫽0. This solution of Eq. 共21兲 has the following simple form, valid for any E(J): ⫽ FIG. 15. Surface plot of E(x,y) distribution around a planar defect for n⫽20. Shown also are the contours of constant E on the xy plane. E 共 0,y 兲 ⬀ 兩 y 兩 n/3. 共71兲 For nⰇ1, the electric field becomes exponentially small in a wide ‘‘shadow’’ region y⬃a 冑n near the defect. For nⰇ1, the length scale of variation of E(0,y) can be obtained by replacing the summation in Eq. 共69兲 by integration, which results in 共see Appendix C兲 冉 冊 E 共 0,y 兲 ⫽E 0 exp ⫺ L 2储 y 2 , L 储 ⫽a 冑 n . 共72兲 This formula gives a good approximation of the exact Eq. 共69兲 for x⬎L 储 共better than 1% for n⬎20). It follows from Eq. 共72兲 that a characteristic length scale L 储 of E(0,y) becomes much greater than a for nⰇ1. For yⰇL 储 , the electric field E(0,y) approaches E 0 as E(0,y)⫺E 0 ⯝n(a/y) 2 E 0 . Notice that the ratio L⬜ /L 储 ⫽ 冑nⰇ1 is in agreement with the general result 共16兲. Although Eq. 共72兲 well describes E(y) for y⬎L 储 , it becomes invalid for y⬍L 储 , where the exponential decrease of E(y) given by Eq. 共72兲 is very different from the exact result E⬀ 兩 y 兩 n/3. Most clearly, this difference manifests itself in current density distributions for y⬍L 储 : instead of the exponential decrease J(y)⬀exp(⫺a2/y2) given by Eq. 共72兲, the exact J(y) exhibits a characteristic cusp of the form J(y)⬀ 兩 y 兩 1/3 共see Fig. 14兲. Shown in Fig. 15 is the spatial distribution of the modulus E(x,y), which reveals characteristic scales of the electricfield variation in all directions. The surface plot of E(x,y) also gives a good approximation for the spatial distribution of local dissipation Q⫽JE near defect for nⰇ1. In this case variations of J(x,y) are week, thus Q(x,y)⫽J 0 E(x,y) to a very good accuracy. The strong, long-range disturbance of E(x,y) near the defect results in a significant excess dissipation, as will be shown below. 共73兲 where the constant A will be obtained below. To calculate z(E, ), we substitute Eq. 共73兲 into Eq. 共34兲 and integrate over , which yields z⫽⫺ J 共 0,y 兲 ⬀ 兩 y 兩 1/3, A sin , E A 2i e ⫹ f 共 E 兲. 2EJ 共74兲 Here f (E) is a real function of E 关the imaginary part vanishes because of the boundary condition y(E,0)⫽y(E, ) ⫽0兴. The equation for f can be obtained by substituting Eqs. 共73兲 and 共74兲 into Eq. 共19兲: E f ⫽ 冉 冊 1 A ⫺ . 2 J 2 E JE 2 共75兲 The boundary condition for f (E) follows from the fact that the electric field E(x,y) becomes infinite at the end of the cut (x⫽y⫽0), as shown in Fig. 6. Then Eq. 共74兲 gives f (⬁)⫽0, and integration of Eq. 共75兲 yields f 共 E 兲 ⫽A 冉冕 ⬁ dE ⬘ E ⫺ JE ⬘ 2 冊 1 . 2JE 共76兲 Equations 共73兲, 共74兲, and 共76兲 give a solution of the nonlinear Maxwell equations, which describe current flow around the half infinite cut for arbitrary J(E). This solution also describes approximately the current flow near the edge of a cut of finite length 2a, where the scaling constant A is determined by the current flow on the length of order a away from the edges. To calculate A we need to match Eq. 共73兲 with the solution of the previous section, which describes current flow around a cut of length 2a, for the power law J(E). To do so we note that for EⰆE c , the power-law approximation is valid everywhere around the cut, except small regions near the ends. Here EⰇE 0 , so the main contribution to comes from the term with k⫽1 and minimum 兩 q ⫺ k 兩 in Eq. 共60兲. This yields the same universal dependence (E, ) ⫽C 1 (E 0 /E)sin as Eq. 共73兲, whence A⫽C 1 E 0 . Using Eqs. 共58兲 and 共63兲, we obtain for nⰇ1 4018 ALEX GUREVICH AND MARK FRIESEN A⫽ 2 5/2h 0 n 3/4E 0 冑 共 n⫹1 兲 ⫽ 4 冑n aJ 0 E 0 . 共77兲 Separating real and imaginary parts of Eq. 共74兲, we get x⫺ f 共 E 兲 ⫽⫺ y⫽⫺ A cos 2 , 2JE L⬜ ⬃anE 0 /E c , 共78兲 共79兲 Thus the contours of constant E are circles of radius A/2JE centered at x⫽ f (E), y⫽0 共Fig. 6兲. Equation 共78兲 and 共79兲 describe the intermediate asymptotics of the current distribution in a small region of radius RⰆa near the edge 共see below兲. Away from the edge, Eqs. 共78兲 and 共79兲 merge with the solution of the previous section, which describes the current flow around the cut and provides the correct asymptotics E→E 0 at infinity. We can further simplify Eq. 共76兲, using the fact that J(E) in superconductors varies rather weakly, even for significant 共by several orders of magnitude兲 changes of E 共see Fig. 1兲. Since the main contribution to the integral in Eq. 共76兲 comes from E ⬘ ⯝E, we can therefore take the slowly varying function J(E ⬘ )⬇J(E) out of the integral and obtain f ⫽A/2JE. 冉 冊 2a 冑n E 0 A ⫽ . R⫽ 2J c E c Ec 共81兲 Excluding from Eqs. 共78兲–共80兲, we obtain the electric-field distribution near the edge: 共 x 2 ⫹y 2 兲 , L 储 ⬃a 冑nE 0 /E c . 共83兲 The condition that the flux flow region is much smaller than a now requires E 0 ⰆE c /n. The hodograph method enables us to trace the evolution of current flow with n and see what happens in the critical state limit, n→⬁. Because of the ambiguity of the Bean model discussed in the Introduction, current flow in the true critical state should be first calculated for large, but finite n values and only then the limit n→⬁ is to be taken. We consider this rather nontrivial limit in detail for current flow past a planar defect, assuming that J 0 ⫽J c at infinity. As was shown before, the solution for J(x,y) describes two regions of current flow, corresponding to J⬍J c and J⬎J c . The solutions for J⬍J c can be obtained from Eqs. 共61兲 straightforwardly, by taking the limit n→⬁. However, the solutions with J⬎J c should be handled with care, since in the Bean model, current densities J⫽J c ⫹0 correspond to infinite E. For J⬍J c , and n→⬁, the stream function described by Eq. 共61兲 can be presented in the following form independent of n: 共80兲 To calculate corrections to f (E) due to flux flow, we assume that J(E)⫽J c ⫹ f E for E⬎E c , where f is the flux flow conductivity. Then the integration of Eq. 共76兲 gives f ⬵A/2J c E⫹A f /2J 2c , if f E/J c Ⰶ1. The radius R of the circular flux flow region near the edge 关 E(x,y)⬎E c 兴 can be obtained by setting E⫽E c in Eqs. 共78兲 and 共79兲 and substituting there Eqs. 共77兲 and 共80兲: E 共 x,y 兲 ⫽ that as E 0 increases, the size of the flux flow region along the x axis, L⬜ , turns out to be much larger than its size, L 储 , along the y axis: B. Critical state limit, n\ⴥ A sin 2 . 2JE 4a 冑nxE 0 PRB 62 x⬎0. 共82兲 The above matching of two solutions near the edge and around the strip is justified, if the radius of the flux flow region R is small compared to the length of the strip 2a. From Eq. 共81兲 we find that RⰆa if E 0 ⰆE c / 冑n. This condition indicates that because of the enhancement of the electric field near the edges, the local flux flow occurs when the bulk E 0 is much smaller than the crossover field E c . However, there is a much stronger applicability condition of the above description, based on the one-term approximation of the sum in Eq. 共62兲. As shown in Appendix C, the terms with k⬎1 in Eq. 共62兲 can be neglected, if E 0 ⰆE f ⬃E c exp(⫺n/8). For E 0 ⰇE f , the flux flow region near the edge becomes noncircular, being essentially stretched out along the x axis 关Fig. 11共a兲兴. An analysis of this case given in Appendix C, shows 8aJ c ⫽ ⬁ 兺 冉冊 J 共 ⫺1 兲 k Jc k k⫽1 4k 2 冉冊 ⬁ z⫽⫺ sin 2k , 16a i 共 ⫺1 兲 k k 2 J e Jc k⫽1 4k 2 ⫺1 兺 共84兲 4k 2 ⫺1 ⫻ 共 cos 2k ⫺2ik sin 2k 兲 . 共85兲 The sums in Eqs. 共84兲 and 共85兲 can be expressed in terms of elliptical theta functions.37 The asymptotics of J(x,y) considerably simplify far away from the defect, ( 兩 z 兩 Ⰷa), as shown in Appendix D. From Eqs. 共85兲, we obtain the current distribution J(y) along the central line x⫽0, ⫽ /2, 16a 兩y兩⫽ ⬁ 兺 k⫽1 k2 冉冊 J 2 4k ⫺1 J c 4k 2 ⫺1 , 共86兲 which is shown in Fig. 14. Near the stagnation point, y→0, the function J(y)⯝J c (3 y/16a) 1/3 exhibits a cusp. Notice that J(y) restores the bulk value J c on the length ⬃a, unlike the electric field E(y), which varies on the scale ⬃a 冑n. The limit n→⬁ cannot be directly taken in the region J ⬎J c , since the sum in Eq. 共62兲 diverges. So we first consider the well-behaved case of large, but finite, n and calculate the boundary between the regions of current flow with E⬎E 0 and E⬍E 0 in the real space 关see Fig. 16共a兲兴. As shown in Appendix D, the boundary is given by the curve y(x), which for nⰇ1 is described parametrically as follows: x⫺a⫽h 0 e ⫺ ␤␥ 冑␥ , 共87兲 NONLINEAR TRANSPORT CURRENT FLOW IN . . . PRB 62 4019 the singular line V 0 ⬃a 冑nE c (J 0 /J c ) n , vanishes. Thus we may ignore the region E⬎E 0 , and Eqs. 共84兲 and 共85兲 give a complete description of the current distribution in the true critical state, E⫽0. Shown in Fig. 16共b兲 are the current streamlines given by Eqs. 共84兲, which are practically indistinguishable from those for large but finite n values in Figs. 11共a兲 and 16共a兲. However, the dc electric field distribution for large but finite n remains very different from the critical state predictions. Indeed, instead of converging to a straight line along the x axes, the region of E⬎E 0 in Fig. 16共b兲 significantly extends along the direction of current flow even for n⫽300, which is much larger than typical values of n ⬃10–50 for superconductors. In the limit, n→⬁, current flow around the defect has the singular d lines, which come out of the stagnation points and extend to infinity as shown in Fig. 16共b兲. Near the stagnation point the d lines make a 45° angle with the x axis and have the same structure as for current flow near the corner, described by Eq. 共50兲. For ( 兩 z 兩 Ⰷa), the following simple equation of the d line can be obtained, as shown in Appendix D: 共89兲 x⫽y 2 /y ⬁ , where y ⬁ ⫽8a/ 冑2 e⬇1.94a. Therefore, far away from the planar defect, the d lines become parabolic, whereas the current streamlines between the d lines in Fig. 15共b兲 are approximately circular, to the accuracy of slowly varying logarithmic factors 共see Appendix D兲. These results are qualitatively similar to current flow around the cylindrical void in the Bean model 共Fig. 4兲. However, unlike Bean’s d line in Fig. 4, current flow near the d lines described by exact Eqs. 共85兲 exhibits no discontinuity in the tangential component of J, thus satisfying the condition ⵜ⫻E⫽0, even in the limit n→⬁. VI. DISSIPATION NEAR PLANAR DEFECTS In this section we obtain a general expression for the excess total dissipation Q due to defects: Q⫽ FIG. 16. Current flow around the planar defect for large 共a兲 and infinite 共b兲 n values, described by Eqs. 共59兲–共63兲 and Eqs. 共84兲 and 共85兲, respectively. The dashed line in Fig. 16共a兲 shows the boundary between the regions of current flow with E⬎E 0 and E⬍E 0 . In the limit n→⬁, this boundary reduces to a ray, y⫽0, shown in 共b兲. The dashed line in 共b兲 shows the d line, which is well described by the parabolic function 共89兲 for x⬎2a. 兩 y 兩 ⫽h 0 冉 1 冑n ␥ 冊 ⫹ 冑␥ e ⫺ ␤␥ , 共88兲 where ␥ ⫽ /2⫺ . From Eqs. 共87兲 and 共88兲, we obtain that 兩 y 兩 ⯝(x⫺a)/ 冑n far away from the defect. In the limit n →⬁, the whole region of E⬎E 0 reduces to a ray along the x axis, where the electric field formally diverges. The voltage across this region, V 0 ⬃E(x)⌬y, is of order E 0 a 冑n, since E(x)⬃E 0 an/(x⫺a), and ⌬y⬃(x⫺a)/ 冑n. In the limit n →⬁, we should take J 0 ⫽J c ⫺0, so that the voltage across 冕 共90兲 dx dy 共 JE⫺J 0 E 0 兲 , where the term J 0 E 0 corresponds to a uniform sample without defects. Now we transform from integration over x and y to the hodograph variables, E and , and obtain 共see Appendix E兲 冕 冕 2 Q⫽ ⬁ d 0 0 冋 共 EJ⫺E 0 J 0 兲 E 共 E 兲 2 ⫹ 册 dE 共 兲2 2 . J J 共91兲 Substituting Eq. 共28兲 into Eq. 共91兲 and integrating over from 0 to 2 , we present Q in the form Q⫽ 冋 兺m C m2 冕0 共 JE⫺J 0 E 0 兲 E 共 E f m 兲 2 ⫹ ⬁ 册 m 2 2 dE f . J m J2 共92兲 Here integration from 0 to 2 implies that current flow contains all possible orientations of J, as it occurs for a planar defect in an infinite superconductor. 4020 ALEX GUREVICH AND MARK FRIESEN We apply these formulas to calculate dissipation power Q, caused by planar defects. We first consider a simpler case of a semi-infinite cut in Fig. 6 and calculate the total dissipation power ⌬Q inside a circular region at the edge where E exceeds a certain electric-field threshold, E c . Substituting Eq. 共73兲 into Eq. 共91兲, we first integrate over from 0 to 共as seen from Fig. 6, the current flow around a semi-infinite, unlike planar defects of finite length, is represented by only half of the hodograph plane, 0⬍ ⬍ ). Integrating then over E, as explained in Appendix E, we obtain a simple exact result, ⌬Q⫽ A 2 /2J c E c , 共93兲 valid for any J-E relation. For instance, if E c is chosen in the flux creep region, ⌬Q is unaffected by the flux flow portion of E(J). Now we calculate Q for a planar defect of length 2a for the power-law E(J) characteristic. Substituting Eq. 共23兲 into Eq. 共91兲 and integrating over E, we obtain ⬁ 冋 册 ⫺ 2 ⫹ 2 q 2m 兩 q 2m⫺1 兩 C 2m⫺1 C 2m E0 , ⫺ Q⫽ 共 n⫹1 兲 ⫺ ⫹ 2J 0 m⫽1 n 兩 q 2m⫺1 兩 ⫹1 nq 2m ⫺1 兺 共94兲 where the subscripts ⫹ and ⫺ corresponds to the signs in front of the square root in Eq. 共32兲. The positive terms, pro2 in Eq. 共94兲, represent an excess dissipaportional to C 2m⫺1 tion due to enhanced electric field around a defect, while the 2 , account for reduced negative terms, proportional to C 2m dissipation in the stagnation regions. For Ohmic conductors, these two opposite contributions exactly cancel each other, giving Q⫽0 for n⫽1 共see Appendix E兲. For nⰇ1, the spatial distribution of Joule dissipation JE is similar to E(x,y) shown in Fig. 15. In this case, there appears an excess dissipation (Q⬎0), since the contribution to Q from the electricfield enhancement along the x axis 共on the scale L⬜ ⬃na) is much greater than the negative contribution of the stagnation regions 共on the scale L 储 ⬃ 冑na). Substituting Eqs. 共58兲 for C m , into Eq. 共94兲 and evaluating the sum as explained in Appendix E, we obtain Q⫽J 0 E 0 a 2 共 n⫺1 兲 冑n. 共95兲 For nⰇ1, Eq. 共95兲 is an exact asymptotics of Q(n), which approximates Eq. 共94兲 to an accuracy better than 1% for n ⬎10 and 6% for 5⬍n⬍10. The physical meaning of Eq. 共95兲 becomes more transparent, by presenting Q in the form Q⯝ L 储 J 0 兰 ⬁a (E⫺E 0 )dx, which is just the excess dissipation in the region of substantial enhancement of E(r) by the defect. Using Eqs. 共64兲 and 共65兲 for E(x), we obtain Q⬃ J 0 E 0 L 储 L⬜ , which gives the correct leading term, Q⯝E 0 J 0 a 2 n 3/2. VII. DISCUSSION The analytical results obtained in this paper reveal essential features of nonlinear 2D current flow, which can affect the current-carrying capability and macroscopic electrodynamics of superconductors. This influence mostly results from the fact that planar obstacles cause strong enhancement and long-range decay of electric-field disturbances. These PRB 62 effects are important for applications, in particular, ac losses, critical state stability, and current flow in thin-film superconducting circuits. The use of the hodograph technique enabled us to address such characteristics of nonlinear current flow, as orientational current flow domains and the structure of current domain walls. In addition, we were able to trace the evolution of current distributions with n and a nonanalytic crossover to the critical state limit, n→⬁, when singular d lines emerge. The fact that a planar obstacle of size a greatly enhances electric-field disturbances over scales L⬜ ⬃an perpendicular to current flow or L 储 ⬃a 冑n along current flow results in long-range interaction between defects, and strong effect of the sample geometry. Indeed, even a sparse network of planar defects can substantially reduce the effective currentcarrying cross section, if the mean spacing between the defects is smaller than L⬃an. For typical values of n⬃30, such a nonlinear blockage of transport current by defects can occur at rather small concentration of obstacles, which occupy only few percent of the geometrical cross section of a superconductor. This effect can have important implications for current percolation through arrays of planar defects, such as grain boundaries in HTS polyscrystals 共Fig. 2兲. It also contributes to multiple current-limiting mechanisms in HTS conductors, such as Bi tapes and biaxially textured YBa2 Cu3 O7 coated conductors.38 For instance, a microcrack, in a film of thickness d 共Fig. 3兲, can cause a strong local peak of E(x) in YBCO coated conductor, even for rather small defects a⬎d/nⰆ1. In turn, such local peaks of voltage and dissipation change the global current-voltage characteristic of the whole conductor, similar to the effect of macroscopic random inhomogeneities.12 A detailed analysis of the significant finite-size effects for current flow in restricted geometries shown in Fig. 3 will be given elsewhere.25 The features of nonlinear current flow discussed above can be observed by the magneto-optical 共MO兲 technique, which indeed revealed long-range disturbances of the normal component of H(x,y) around macroscopic defects in HTS’s.7,9 For instance, characteristic flamelike shapes of the magnetic-flux disturbances around defects on MO images are similar to the contours of constant E shown in Figs. 11 and 15. By measuring the scales L⬜ and L 储 of magnetic-flux disturbance, one can extract both the n value, n⯝(L⬜ /L 储 ) 2 , and the size of the defect, a⬃L⬜ /n, even if the defect is smaller than the MO resolution 共usually ⯝50–10 m). Extensive stagnation regions (L 储 ⬃a 冑n) of exponentially small electric field constitute another feature of nonlinear current flow around planar defects 关Fig. 11共a兲兴 which could be observed in MO experiments. This nonlinear ‘‘shadow effect’’ manifests itself in the distribution of flux velocities, v⫽ 关 H0 ⫻E兴 /H 20 , in a strong magnetic field H 0 when vortices move along equipotential lines, (x,y)⫽const. Vortex velocity v sharply increases in the regions of enhanced electric field near the edges of the planar defect, which thus becomes a flow channel for magnetic flux 关see Figs. 11共a兲 and 15兴. These flux jets are sandwiched between two macroscopic stagnation regions of nearly motionless flux which result from the geometry of the current flow and the strong nonlinearity of E(J), but are not due to enhanced flux pinning. PRB 62 NONLINEAR TRANSPORT CURRENT FLOW IN . . . The excess dissipation Q caused by defects is another important feature of the strong nonlinearity of E(J). Superconducting materials, and especially HTS’s, contain many macroscopic current-limiting defects 共microcracks and highangle grain boundaries兲,6 which contribute significantly to the overall ac losses and dissipation. As an example, we consider a sparse array of planar defects of size ⬃a spaced by lⰇa. Then we obtain from Eq. 共95兲 that the defects result in the excess dissipation power ⬃n 3/2(a/l) 2 J 0 E 0 per unit volume, which becomes of the order of the background bulk dissipation power J 0 E 0 , if l⬍an 3/4. Therefore the overall dissipation will be dominated by defects, if they occupy a rather small fraction ⬃n ⫺3/4 of the geometrical cross section of the sample 共few percent for the typical n values ⬃20–30 for superconductors兲. The excess dissipation due to defects can also trigger local thermal instabilities in high-J c superconductors.36 Such instabilities develop mostly in the regions of enhanced heat generation E⬎E 0 in Figs. 11共a兲 and 15, which dominate the overall Q. Another type of orientational current instabilities can be caused by the high anisotropy of HTS’s,21 when current is forced to flow along the c axis by microcracks8 or a ‘‘brick-wall’’ structure of inplane tilt grain boundaries.39 ACKNOWLEDGMENTS Another feature of Ohmic conductors is that the complex potential w(u) is also an analytic function in the hodograph plane, u⫽ ⫺i , where ⫽ln(E/E0). In nonlinear conductors, depends on E, so neither w(z) nor w(u) are analytic functions. We consider properties of w for the power law E(J), for which Eqs. 共20兲 can be written in the following symmetric form: ⫽ 共 0 / 冑n 兲 e 2 ␤ , 共A5兲 ⫽⫺ 共 0 / 冑n 兲 e 2 ␤ , 共A6兲 where ␤ ⫽(n⫺1)/2冑n, ⫽n ⫺1/2 ln(E/E0), and 0 ⫽E 0 /J 0 . Defining new functions, h 1 ⫽ exp(⫺␤) and h 2 ⫽( 冑n/ 0 ) exp(␤), we present Eqs. 共A5兲 and 共A6兲 in the form 2D current flow in Ohmic conductors is described by the complex potential w 共 z 兲 ⫽ ⫺i , 共A1兲 which is an analytic function of z⫽x⫹iy. The analyticity of w(z) greatly simplifies the calculation of 2D current distributions, allowing exact solutions for the geometries shown in Fig. 3 to be obtained using conformal mapping.32 The condition that w(z) is an analytic function can be written in the form dw dz̄ ⫽0, 共A2兲 where the bar denotes complex conjugate, and the complex differentiation of any function f (z)⫽u⫹i v is defined as34 冉 冊 冉 冊 1 u v i v u ⫽ ⫹ . ⫺ ⫹ 2 x y 2 x y dz̄ df The fact that d f /dz̄⫽0 for any analytic function f (z) follows from the Cauchy-Riemann conditions, x u⫽ y v , y u ⫽⫺ x v . The electric-field distribution, E x ⫹iE y ⫽E exp(i), can be calculated from Ee ⫺i dw ⫽⫺ . dz 共A4兲 共A7兲 h 1⫹ h 1⫽ ␤ h 2 . 共A8兲 ␤ ⫽⫺ w̄ 0 , 2 dū dw 0 共A9兲 which describes generalized analytic functions.33 Therefore calculations of current flow in nonlinear conductors can be formulated in terms of generalized analytic functions for the effective potential w 0 (u) in the hodograph plane, u⫽ ⫺i . This fact enables one to calculate 2D nonlinear current flow by constructing an appropriate generalized analytical function,22 using methods which have been developed in the literature.33 Expressing w 0 in terms of and , we obtain w 0⫽ e ⫺␤⫺ i0 冑n e ␤ . 共A10兲 For n⫽1, the effective potential w 0 reduces to w. APPENDIX B: NORMALIZATION CONSTANT To calculate h 0 , we equate Eqs. 共61兲 and 共62兲 to obtain the self-consistency condition z(⫹0,0)⫽z(⫺0,0), whence a⫽⫺ 共A3兲 h 1 ⫺ h 2 ⫽⫺ ␤ h 1 , These equations can be combined into a single complex equation for the effective complex potential, w 0 ⫽h 1 ⫺ih 2 . Using complex differentiation 共A3兲 with respect to u⫽ ⫺i , we obtain the equation for w 0 in the form of a firstorder Carleman equation, We are grateful to D. C. Larbalestier and A. P. Malozemoff for discussions. This work was supported by the NSF MRSEC 共Grant No. DMR 9214707兲 and EPRI. APPENDIX A: ANALYTIC PROPERTIES OF THE COMPLEX POTENTIAL 4021 1 ⬁ 兺 J 冑n k⫽1 0 冉 冊 2k 2k⫺1 C 2k ⫹ C 2k⫺1 . uk pk 共B1兲 It is convenient to write Eq. 共B1兲 as h 0 ⫽⫺aJ 0 /I, where I is obtained from Eqs. 共57兲 and 共58兲 in the form I⫽ 2 3/2 ⬁ 兺 冑 n m⫽1 ⫹ 冋 2m 共 ⫺1 兲 m 冑␣ 2m ⫺ ␤ 共 4m ⫺1 兲 ␣ 2m 2 共 2m⫺1 兲共 ⫺1 兲 m 冑␣ 2m⫺1 ⫹ ␤ ␣ 2m⫺1 共 ␣ 2m⫺1 ⫹ ␤ ⫹1/冑n 兲 册 冉 . ␣ 2m ⫹ ␤ ⫹ 1 冑n 冊 共B2兲 4022 ALEX GUREVICH AND MARK FRIESEN For nⰇ1, this sum is dominated by the first term in the square brackets, where 1/冑n in ( ␣ 2m ⫹ ␤ ⫹1/冑n) can be neglected. Then I reduces to I⫽ 2 3/2 ⬁ 兺 共 ⫺1 兲 m 冑 n m⫽1 冉 冑␣ 2m ⫹ ␤ 共 4m ⫺1 兲 ␣ 2m 2 ⫹ 冑␣ 2m ⫹ ␤ ␣ 2m 冊 . 共B3兲 The first part of this sum, I 1 , is rapidly converging over m ⬃1, so the slowly varying factor 冑␣ 2m ⫹ ␤ / ␣ 2m can be replaced by its constant value at m⫽1. Then the summation yields I 1 ⫽⫺ ⫺2 冑 n ␤ 共B4兲 . The second part of I is an expression of the form I 2 ⬁ ⫽ 兺 m⫽1 (⫺1) m F m , where F m , given by the second term in the square brackets, decreases slowly with m for nⰇ1. To turn I 2 into a rapidly converging series, we write ⬁ I 2⫽ ⬁ ⬁ 1 兺 共 F 2m ⫺F 2m⫺1 兲 ⫽ m⫽1 兺 k⫽1 兺 2 k k! m⫽1 d k F 2m dm k , 共B5兲 where F m is nearly constant for m⬍ ␤ , and decreases as 1/冑m for m⬎ ␤ . Therefore each differentiation of F m over m brings a small factor ⬃1/冑n, so the main contribution to I 2 comes from the term with k⫽1. Since dF m /dm is a slow function of m, we can replace summation in Eq. 共B5兲 by integration using the Poisson-Euler formula34 written in the form 兺 f 共 m 兲 ⬇ 冕0 f 共 x 兲 dx⫺ m⫽1 ⬁ ⬁ f 共0兲 m f 共0兲 ⫺ , 2 12 共B6兲 where f m ⫽0.5dF m /dm. Since F m is a function of m 2 , the second term in the right-hand side of Eq. 共B6兲 vanishes, and the last term ⬃ ␤ ⫺5/4Ⰶ1 is negligible. As a result, the sum 共B6兲 equals ⫺F 0 /2, thus I 2 ⫽⫺ 2 冑 n ␤ 共B7兲 . Combining I 1 and I 2 , we obtain Eq. 共63兲, which approximates Eq. 共B1兲 to the accuracy better than 1% for n⬎5. APPENDIX C: ASYMPTOTICS OF z„E, … To sum up Eq. 共69兲 at nⰇ1, we consider the region of x⬍a 冑n, where EⰆE 0 . The convergence of the sum is then mostly determined by the factors (E 0 /E) k , where k ⫽( ␣ 2k ⫺ ␤ )/ 冑n⫺1/n. In this case the main contribution to Eq. 共69兲 for nⰇ1 comes from the region k⬍ ␤ , where the slowly varying factor ␣ 2k can be taken out of the sum at k ⫽1. Then ␣ 2k ⫺ ␤ ⬇2k 2 / ␤ , k ⬇4k 2 /n, and Eq. 共69兲 reduces to y⫽ 4a ⬁ 兺 k⫽1 冉 冊 E E0 4k 2 /n . 共C1兲 PRB 62 For nⰇ1, the sum in Eq. 共C1兲 can be evaluated with the use of Eq. 共B6兲, giving 关 n/ln(E/E0)兴1/2/4. As a result, we arrive at Eq. 共72兲. This approach gives the intermediate asymptotics of E(0,y) at y⬃L 储 . The behaviors of E(0,y) for y→⬁ should be obtained in a different way, since for E→E 0 , the sum in Eq. 共69兲 diverges. The main contribution then comes from kⰇ ␤ , and Eq. 共69兲 becomes y⫽ ⬁ a 1 兺 冑2n 1/4 k⫽1 冑k 冉 冊 E E0 2k/ 冑n 共C2兲 . For nⰇ1, evaluation of this sum with the use of Eq. 共B6兲, gives y⫽a 冑n/ ln⫺1/2(E 0 /E). This yields the same asymptotic behavior of E(0,y)⫺E 0 ⫽E 0 (L 储 /y) 2 as Eq. 共72兲. To calculate the distribution of E(x,y) near the edges, we write Eq. 共62兲 in the form z⫺a⫽ 2 3/2h 0 e i 冑 J 0 ⫻ 冋 ⬁ 兺 k⫽1 2k⫺1 冑n 冉 冊 共 ⫺1 兲 k 冑␣ 2k⫺1 ⫹ ␤ E 0 p k ␣ 2k⫺1 E k cos共 2k⫺1 兲 册 ⫹i 共 ␣ 2k⫺1 ⫹ ␤ 兲 sin共 2k⫺1 兲 , 共C3兲 where k ⫽ 兩 q 2k⫺1 兩 ⫹1/n. Near the edges, where EⰇE 0 , the convergence of this sum is determined by the small factor (E 0 /E) k ⫽exp关⫺k ln(E/E0)兴 at (2k⫺1) 2 ⬍n. There are two characteristic domains. The first one is very close to the edge (E→⬁), so that the sum 共C3兲 is dominated by the term k⫽1, for which the exponent 1 ⫽1⫹1/n is minimum. In this case the term with k⫽2 is negligible, that is, exp关⫺(2 ⫺1)ln(E/E0)兴Ⰶ1. For nⰇ1, we get 2 ⫽1⫹9/n, thus the sum in Eq. 共C3兲 is determined by only one term with k⫽1, if (8/n)ln(E/E0)⬎1. This criterion defines the size of the region, r c ⬃a 冑n exp(⫺n/8), at the edge, where the one-term approximation holds. Since r c decreases exponentially with n, there is a wide region near the planar defect where ln(E/E0)Ⰷ1, but the terms with k⬎1 in Eq. 共C3兲 cannot be neglected. In the large region r c ⰆxⰆan, where EⰇE 0 , the convergence of the sum 共C3兲 is mostly determined by the factor (E 0 /E) k , while the much weaker k dependence of ␣ 2k⫺1 can be neglected. In this case we can replace ␣ 2k⫺1 ⬇ ␤ and expand k ⬇1 ⫹(2k⫺1) 2 /n. As a result, Eq. 共C3兲 for nⰇ1 reduces to z⫺a⫽ 冉 冊冉 冊 2 5/2h 0 e i E 0 冑 n 1/4J 0 E I⬘ ⫹I , n 共C4兲 ⬁ I共 , 兲⫽ 兺 k⫽1 2 共 ⫺1 兲 k e ⫺ (2k⫺1) sin共 2k⫺1 兲 . 共C5兲 Here ⫽n ⫺1 ln(E/E0), I ⬘ ⫽ I, and I( , ) can be expressed in terms of elliptical theta-functions.37 Notice that I( , ) satisfies the ‘‘diffusion’’ equation I⫽ I. 共C6兲 PRB 62 NONLINEAR TRANSPORT CURRENT FLOW IN . . . Separating real and imaginary parts of Eq. 共C4兲, we express x( , ) and y( , ) in terms of I( , ): where ␥ ⫽ /2⫺ , and x⫺a⫽l 关共 I ⬘ /n 兲 cos ⫺I sin 兴 , 共C7兲 ⫽ y⫽l 关共 I ⬘ /n 兲 sin ⫹I cos 兴 , 共C8兲 where l⫽(4a 冑n/ )(E 0 /E c ). To calculate I( , ), we multiply Eq. 共C5兲 by sin(2m⫺1) and integrate from 0 to /2: 冕 /2 0 ⫺(2m⫺1) 2 e , 4 I cos共 2m⫺1 兲 ␥ d ␥ ⫽ 共C9兲 where ␥ ⫽ /2⫺ . We consider the wide region of E, where ln(E/E0)⬎1, but Ⰶ1. The main contribution to the integral in Eq. 共C9兲 then comes from ␥ Ⰶ1, so we can extend the upper integration limit to ⬁ and obtain I共 ␥, 兲⫽ 冑 ⫺ ␥ 2 /4 e . 4 冑 共C10兲 This is a well-known solution of the diffusion Eq. 共C6兲, which describes the evolution of I( ␥ , ) in an infinite 1D media after applying a pulse ⬀ ␦ ( ␥ ) ␦ ( ).34 Substituting Eq. 共C10兲 into Eqs. 共C7兲 and 共C8兲 and using the fact that ␥ Ⰶ1, we obtain the distribution E(x,y) in the following parametric form: y⫽ 关 1⫹1/2 ln共 E/E 0 兲兴 l ␥ I. x⫺a⫽lI, 共C11兲 h 0e ⫺␤ g⫽ 2 冑n 冉 ln1/2共 E c /E 0 兲 1⫹ L⬜ ⫽ 共C12兲 冊 1 , 2 ln共 E c /E 0 兲 冉 冊 E0 . 冑 ln 共 E c /E 0 兲 E c an 1/2 共C13兲 共C14兲 The contour y(x) shown in Fig. 11共a兲 is quite different from the circular flux flow regions of the k⫽1 approximation. Here the length L⬜ of the domain with E⬎E c along the x axis becomes much larger than its size L 储 along the y axis. Indeed, the maximum of y(x)⫽L 储 occurs at x⫽L⬜ / 冑e. Substituting this into Eq. 共C12兲, we obtain L 储 ⫽a 冑 冋 2n 1 1⫹ e 2 ln共 E c /E 0 兲 册冉 冊 E0 . Ec 共C15兲 To the accuracy of slowly varying logarithmic terms, we again arrive at the universal relation L⬜ ⬃ 冑nL 储 . APPENDIX D: CRITICAL STATE LIMIT To calculate the boundary ( ⫽0) between the regions E⬍E 0 and E⬎E 0 , we integrate Eq. 共34兲, written in the form ␥ x⫽⫺ 共 cos ␥ ␥ ⫹n ⫺1/2 sin ␥ 兲 e ⫺ / 冑n /J 0 , 共D1兲 ␥ y⫽ 共 sin ␥ ␥ ⫺n ⫺1/2 cos ␥ 兲 e ⫺ / 冑n /J 0 , 共D2兲 关 冑 2 ⫹ ␥ 2 ⫹ 兴 1/2. 共D3兲 After differentiating Eq. 共D3兲 in Eqs. 共D1兲 and 共D2兲, we set ⫽0. From the form of for ␤ Ⰷ1, it follows that the main contribution in Eqs. 共D1兲 and 共D2兲, comes from ␥ Ⰶ1. This allows us to expand sin␥ and cos␥ in ␥ , retaining only linear and quadratic terms. Then integration of Eqs. 共D1兲 and 共D2兲 from ␥ to ⬁, with the boundary conditions x(⬁)⫽a,y(⬁) ⫽0, yields x⫽a⫹ y⫽ h 0 e ⫺ ␤␥ J0 冉 h 0 e ⫺ ␤␥ J 0 冑␥ 1 冑n ␥ ⫺ h 0 冑2 J 0 n 3/4 冊 erfc冑␤␥ , 3 冑2 h 0 ⫹ 冑␥ ⫹ 4J 0 n 5/4 共D4兲 erfc冑␤␥ . 共D5兲 These formulas determine parametrically the boundary y(x) of the region of enhanced dissipation (E⬎E 0 ) around the planar defect. For nⰇ1, the terms proportional to the error function erfc(x) can be neglected, which gives Eqs. 共87兲 and 共88兲. Now we calculate J(x,y) far away from the defect. To sum up Eq. 共85兲, we present it in the form z⫽⫺be i 共 I 0 ⫹iI ⬘0 兲 , ⬁ L⬜ , x⫺a 冑 2 ⫹ ␥ 2 ⫺ ␤ 冑 2 ⫹ ␥ 2 Excluding ␥ from Eq. 共C11兲, we obtain contours of equal E(x,y)⫽E c : 兩 y 兩 ⫽g 共 x⫺a 兲 ln1/2 4023 I 0⫽ 兺 k⫽1 共 ⫺1 兲 k k 2 k ⫺1/4 2 e ⫺(4k 2 ⫺1) 共D6兲 cos 2k , 共D7兲 where I ⬘0 ⫽ I 0 , b⫽4a/ , and ⫽ln(Jc /J)⬎0. We consider J(x,y) for 兩 z 兩 Ⰷa, where J→J c , thus Ⰶ1. In this case I 0 reduces to ⬁ I 0⫽ 兺 k⫽1 2 e ⫺4k cos 2k ␥ ⫹ 1 4 ⬁ cos 2k ␥ , 兺 k⫽1 k 2 ⫺1/4 共D8兲 where the complimentary angle ␥ (x,y)⫽ /2⫺ is small 共see Fig. 15兲. The second sum is rapidly converging, so we 2 omitted the factor e ⫺4k , inessential for Ⰶ1. The first sum is calculated using Eq. 共B6兲, and the second sum equals 2 ⫺ sin ␥. Hence I 0⫽ I ⬘0 ⫽ 冑 ⫺ ␥ 2 /4 e ⫺ sin ␥ , 4 4 冑 冑 ␥ 8 e ⫺␥ 3/2 2 /4 ⫹ cos ␥ . 4 共D9兲 共D10兲 Combining Eqs. 共D6兲 and 共D10兲, we obtain the following parametric description of z( , ␥ ): x⫽⫺b 共 sin ␥ I 0 ⫺cos ␥ I ⬘0 兲 , 共D11兲 y⫽⫺b 共 cos ␥ I 0 ⫹sin ␥ I 0⬘ 兲 . 共D12兲 4024 ALEX GUREVICH AND MARK FRIESEN To reveal the d lines, we calculate the function ␥ (x,y) from Eqs. 共D11兲 and 共D12兲, expressing for xⰇa,y⬍0 as follows: ⫽⫺ ␥ 关 x sin ␥ ⫹y cos ␥ 兴 . 2 关 x cos ␥ ⫺y sin ␥ 兴 冋 共 1⫹ ␥ 兲 册 ␥ 共 1⫹ ␥ 兲 ⫽ exp ⫺ , 2 3 ⫺␥ b 共⫺␥兲 ␥ 8x 2 共D14兲 which determines ␥ (x,y) as a function of x and ⫽⫺y/x. Now we find the position of the d line, on which the spatial derivatives of ␥ (x,y) diverge. Considering Eq. 共D14兲 as an explicit expression of the form x⫽x( , ␥ ), we conclude that ␥ x⫽0, that is, the gradient of ␥ along the line y⫽⫺ x diverges on the d line. Differentiating Eq. 共D14兲 over ␥ for ⫽const, we obtain that the condition ␥ x⫽0 gives ␥ ⫽ /2. Substituting this back into Eq. 共D14兲, we arrive at Eq. 共89兲. APPENDIX E: DISSIPATION To transform from integration over dxdy to the hodograph variables in Eq. 共90兲, we write dxdy⫽Wd dE, where the Jacobian, W⫽ x E y⫺ y E x, is calculated using Eqs. 共34兲 and 共35兲. This yields W⫽ 冉 1 J 2 E共 E 兲2⫹ 冊 共 兲2 . J 共E1兲 The value Q does not change sign for any isotropic J(E) with a positive differential conductivity, ⫽ J/ E. This fact makes the hodograph transformation a single-valued procedure, that is, a given solution (E, ) corresponds uniquely to physical distributions of E and J in the coordinate space xy. To calculate ⌬Q in the flux flow region near the edge of a half infinite cut, we substitute ⫽A sin /E in Eq. 共91兲 and integrate over from 0 to : ⌬Q⫽ 2 A 2 冕冉 ⬁ 1⫹ Ec 冊 E dE . J JE 2 ⬁ Ec dE 2 J E ⫽ 1 ⫺ E cJ c 冕 ⬁ dE E c JE 2 . Q⫽ J0 ⫺ 冉 冊兺 冉 1 1⫹ n ⬁ m⫽1 共 ␣ 2m⫺1 ⫹ ␤ 兲 2 2 ␣ 2m⫺1 共 ␣ 2m⫺1 ⫹ ␤ ⫹1/冑n 兲 共 ␣ 2m ⫺ ␤ 兲 2 2 ␣ 2m 共 ␣ 2m ⫺ ␤ ⫺1/冑n 兲 冊 . 兺 J0 m⫽1 冋冉 冊 冉 1 1 1 1 ⫺ ⫹␤ 2 ⫹ 2 ␣ 2m⫺1 ␣ 2m ␣ 2m⫺1 ␣ 2m 共E4兲 冊册 , 共E5兲 where ␣ m ⫽ 冑m 2 ⫹ ␤ 2 . Expanding 1/␣ 2m⫺1 ⬇1/␣ 2m ⫺0.5 m (1/␣ 2m ) in the first parentheses and using Euler’s formula 共B6兲, we obtain that the sum of the first term in the square brackets equals 1/2␣ 0 ⫽1/2␤ . The summation of the second term in the square brackets yields /2⫺1/2␤ . Combining these two contributions, we obtain Q⫽2 E 0 h 20 /J 0 ⫽a 2 J 0 E 0 n 3/2, 共E6兲 where we used Eq. 共63兲 for h 0 . Equation 共E6兲 gives the leading term in the expansion of Q(n) in nⰇ1. In Eq. 共95兲 we also took into account the next term of order a 2 J 0 E 0 冑n, obtained from the best fit of the full dependence Q(n) given by Eq. 共E4兲. Eq. 共95兲 not only well describes the exact Q(n), but also provides the correct limit Q⫽0 for n⫽1. In conclusion, we calculate Q for a planar defect in Ohmic conductors (n⫽1). It is instructive to do so using Eq. 共51兲, which gives the complex electric field E exp(⫺i) ⫽⫺dw/dz in the form Ee ⫺i ⫽⫺i zE 0 冑z 2 ⫺a 2 共E7兲 . Substituting Eq. 共E7兲 into Eq. 共90兲, we obtain Q ⫽ Q0 冕 ␣冕 2 d 0 c 0 冋 2 冑 4 ⫺2 2 cos 2 ␣ ⫹1 册 ⫺1 d , 共E8兲 where Q 0 ⫽ E 20 a 2 , x⫽a cos ␣, y⫽a sin ␣. To avoid the formally diverging integral in the brackets, we introduce an auxiliary constant c Ⰷ1 and obtain after integration over in the limit c →⬁: 共E3兲 After substituting Eq. 共E3兲 into Eq. 共E2兲, the integral terms cancel out and we arrive at Eq. 共93兲. To calculate Q for a planar defect, we present Eq. 共94兲 in the form 4E 0 h 20 Q⫽ ⬁ 4E 0 h 20 共E2兲 Integrating the second term in the brackets by parts, we obtain 冕 For nⰇ1, the terms in the brackets decay rather slowly with m, so the main contribution to the sum comes from mⰇ1. In this case we can neglect 1/冑n in the denominators and rewrite Eq. 共E4兲 in the form 共D13兲 Substituting Eq. 共D13兲 into Eqs. 共D11兲 and 共D12兲, and expanding in ␥ Ⰶ1, we obtain the following relation: PRB 62 Q⫽Q 0 冕 0 关 cos 2 ␣ ln共 2 2c /e 兲 ⫺cos 2 ␣ ln共 1⫺cos 2 ␣ 兲 ⫺1 兴 d ␣ . 共E9兲 The term proportional to ln c vanishes after integration over ␣ . Integrating the second term in Eq. 共E9兲 by parts, we obtain that it cancels the contribution from the last term in the integrand, giving Q⫽0. Thus a planar defect in an infinite Ohmic conductor does not cause any excess overall dissipation. In this case excess dissipation at the edges is exactly compensated by reduced dissipation in stagnation regions. PRB 62 1 NONLINEAR TRANSPORT CURRENT FLOW IN . . . G. Blatter, M.V. Feigelman, V.B. Geshkenbein, A.I. Larkin, and V.M. Vinokur, Rev. Mod. Phys. 66, 1125 共1994兲. 2 E.H. Brandt, Rep. Prog. Phys. 58, 1465 共1995兲. 3 Y. Yeshurun, A.P. Malozemoff, and A. Shaulov, Rev. Mod. Phys. 68, 911 共1996兲. 4 A. Gurevich and H. Küpfer, Phys. Rev. B 48, 6477 共1993兲; A. Gurevich, Int. J. Mod. Phys. B 9, 1054 共1995兲; A. Gurevich and E.H. Brandt, Phys. Rev. Lett. 73, 178 共1994兲; E.H. Brandt, ibid. 76, 4030 共1996兲. 5 C.J. van der Beek, P.H. Kes, M.R. Maley, M.J.V. Menken, and A.A. Menovsky, Physica C 195, 307 共1992兲; A.A. Zhukov, H. Küpfer, V.A. Ryabchuk, L.A. Ponomarenko, V.A. Murashov, and Yu. A. Martynkin, ibid. 219, 99 共1994兲; M. Nideröst, A. Suter, P. Visani, A.C. Mota, and G. Blatter, Phys. Rev. B 53, 9286 共1996兲. 6 D.C. Larbalestier, Science 274, 736 共1996兲; IEEE Trans. Appl. Supercond. 7, 90 共1997兲. 7 A.E. Pashitski, A. Gurevich, A.A. Polyanskii, D.C. Larbalestier, A. Goyal, E.D. Specht, D.M. Kroeger, J.A. DeLuca, and J.E. Tkaczykl, Science 275, 367 共1997兲; A. Polyanskii, A. Pashitski, A. Gurevich, J.A. Parrel, M. Polak, D.C. Larbalestier, S.R. Foltyn, and P.N. Arendt, Adv. Supercond. 9, 469 共1997兲. 8 M. Polak, J.A. Parrell, A.A. Polyanskii, A.E. Pashitski, and D.C. Larbalestier, Appl. Phys. Lett. 70, 1034 共1997兲; X.Y. Cai, A. Polyanskii, Q. Li, G.N. Riley, and D.C. Larbalestier, Nature 共London兲 392, 906 共1998兲. 9 Th. Schuster, T. Kuhn, E.H. Brandt et al., Phys. Rev. B 52, 10 375 共1995兲; 54, 3514 共1996兲; 56, 3413 共1997兲. 10 V.K. Vlasko-Vlasov, G.W. Crabtree, U. Welp, and V.I. Nikitenko 共unpublished兲. 11 J.P. Clerc, G. Giraud, J.M. Laugier, and J.M. Luck, Adv. Phys. 39, 191 共1990兲; M.B. Isichenko, Rev. Mod. Phys. 64, 961 共1992兲. 12 A. Gurevich and V.M. Vinokur, Phys. Rev. Lett. 83, 3037 共1999兲. 13 A. Gurevich, Fiz. Tverd. Tela 共Leningrad兲 30, 1384 共1988兲 关Sov. Phys. Solid State 30, 800 共1988兲兴; Phys. Rev. B 42, R4857 共1990兲; A. Gurevich, H. Küpfer, and C. Keller, Europhys. Lett. 15, 789 共1991兲. 14 J. Straley and S. Kenkel, Phys. Rev. B 29, 6299 共1984兲; E. Hinrichsen, S. Roux, and A. Hansen, Physica C 167, 433 共1990兲; P.L. Leath and W. Xia, Phys. Rev. B 44, 9619 共1991兲; R. Haslinger and R. Joynt, ibid. 61, 4206 共2000兲. 15 A. Goyal, E.D. Specht, D.M. Kroeger, and T.A. Manson, Appl. Phys. Lett. 68, 711 共1996兲; E.D. Specht, A. Goyal, and D.M. Kroeger, Phys. Rev. B 53, 3585 共1996兲. 16 V.M. Vinokur, M.V. Feigelman, and V.B. Geshkenbein, Phys. Rev. Lett. 67, 915 共1991兲. 17 E.H. Brandt, Phys. Rev. B 54, 3530 共1996兲; 54, 4246 共1996兲; 55, 14 513 共1997兲; 58, 6506 共1998兲; 58, 6523 共1998兲; 59, 3369 共1999兲. 18 C.P. Bean, Rev. Mod. Phys. 36, 31 共1964兲. 19 A.M. Campbell and J.E. Evetts, Adv. Phys. 21, 1191 共1972兲. 20 4025 Th. Schuster, H. Kuhn, and M.V. Indenbom, Phys. Rev. B 52, 15 621 共1995兲. 21 A. Gurevich, Phys. Rev. B 46, 3638 共1992兲. 22 A. Gurevich and J. McDonald, Phys. Rev. Lett. 81, 2546 共1998兲. 23 S.A. Chaplygin, On Gas Jets 共Brown University, Providence, RI, 1944兲; L.I. Sedov, Two-Dimensional Problems in Hydrodynamics and Aerodynamics 共Interscience, New York, 1965兲. 24 L.D. Landau and E.M. Lifshits, Fluid Mechanics 共Pergamon, Oxford, 1987兲; L.M. Milne-Thompson, Theoretical Aerodynamics 共Dover, New York, 1973兲. 25 M. Friesen and A. Gurevich 共unpublished兲. 26 K. Seeger, Semiconductor Physics 共Springer-Verlag, Berlin, 1982兲. 27 W.T. Norris, J. Phys. D 3, 489 共1970兲. 28 J.R. Clem, R.P. Huebener, and D.E. Gallus, J. Low Temp. Phys. 12, 449 共1973兲. 29 E. Zeldov, A.I. Larkin, V.B. Geshkenbein, M. Konczykowski, D. Mayer, B. Khaykovich, V.M. Vinokur, and H. Shtrikman, Phys. Rev. Lett. 73, 1428 共1994兲. 30 E. Zeldov, J.R. Clem, M. McElfresh, and M. Darwin, Phys. Rev. B 49, 9802 共1994兲. 31 E.H. Brandt and M.V. Indenbom, Phys. Rev. B 48, 12 893 共1994兲. 32 L.D. Landau and E.M. Lifshits, Electrodynamics of Continuous Media, Theoretical Physics Vol. VIII 共Pergamon, Oxford, 1963兲. 33 I.N. Vekua, Generalized Analytical Functions 共Pergamon, London, 1962兲. 34 P.M. Morse and H. Feshbach, Methods of Theoretical Physics 共McGraw-Hill, New York, 1953兲. 35 Equations 共57兲–共63兲 were obtained for nⰇ1, so they do not reduce to the Ohmic case (n⫽1), described by Eqs. 共51兲 and 共52兲. However the discrepancy between Eqs. 共57兲–共63兲 and the exact solution becomes exponentially small for n⬎3, since the accuracy of Eqs. 共57兲–共63兲 is of order exp(⫺␤)Ⰶ1. The discrepancy manifests itself as a mismatch of two exact hodograph solutions ⫹ (x,y) and ⫺ (x,y) at the contour E(x,y)⫽E 0 , which separates the regions of current flow with E⬎E 0 and E ⬍E 0 , respectively. This mismatch is visible at n⬍3, but becomes undetectable in Figs. 11–16, which correspond to n⬎3. 36 A.V. Gurevich, R.G. Mints, and A.L. Rakhmanov, The Physics of Composite Superconductors 共Begell House, New York, 1997兲. 37 Handbook of Mathematical Functions, Applied Mathematics Series Vol. 55, edited by M. Abramowitz and I.R. Stegun 共National Bureau of Standards, Washington, DC, 1964兲. 38 X.D. Wu, S.R. Foltyn, P.N. Arendt, W.R. Blumenthal, I.H. Campbell, J.D. Cotton, J.Y. Coulter, W.L. Hults, M.P. Maley, H.F. Safar, and J.L. Smith, Appl. Phys. Lett. 67, 2397 共1995兲; D.P. Norton, A. Goyal, J.D. Budai, D.K. Christen, D.M. Kroeger, E.O. Specht, Q. He, B. Saffian, M. Paranthaman, C.E. Klabunde, D.F. Lee, B.C. Sales, and F.A. List, Science 274, 755 共1996兲. 39 L.N. Bulaevskii, J.R. Clem, L.I. Glazman, and A.P. Malozemoff, Phys. Rev. B 45, 2545 共1992兲.